Hu 09007dcc805d8846

Upload
siavoshani 
Category
Documents

view
353 
download
5
description
Transcript of Hu 09007dcc805d8846
MODELING AND SIMULATION OF HIGH PRESSURE COMPOSITE
CYLINDERS FOR HYDROGEN STORAGE
by
JIANBING HU
A DISSERTATION
Presented to the Faculty of the Graduate School of the
MISSOURI UNIVERSITY OF SCIENCE AND TECHNOLOGY
In Partial Fulfillment of the Requirements for the Degree
DOCTOR OF PHILOSOPHY
IN MECHANICAL ENGINEERING
2009
Approved by
K. Chandrashekhara, Advisor Lokeswarappa R. Dharani
HaiLung Tsai Gregory E. Hilmas
William E. Showalter
2009
Jianbing Hu
All Rights Reserved
iii
PUBLICATION DISSERTATION OPTION
This dissertation has been prepared in the form of three papers for publication as
follows:
Pages 747 have been published in ADVANCED COMPOSITE MATERIALS.
Pages 4887 have been published in INTERNATIONAL JOURNAL OF HYDROGEN
ENERGY.
Pages 88128 intended to submit to INTERNATIONAL JOURNAL OF HYDROGEN
ENERGY.
iv
ABSTRACT
Composite hydrogen cylinders provide an efficient means of storage of hydrogen gas
for modern hydrogen vehicles. Safety issues arising from the high gas pressure,
temperature variation, fire attack, and fracture failures are the main concerns. The focus
of this study is to develop a Finite Element (FE) model to predict the performance of
composite cylinders subjected to extreme mechanical/thermal loadings and provide
guidance for design optimization. In the first part of this work, a predictive FE model of
composite cylinders has been developed considering various mechanical and thermal
loadings. Doublycurved laminated shell theory, accounting for transverse shear
deformation and geometric nonlinearity, is used to model the composite cylinder wall. A
backpropagation Neural Network (NNk) model, which is capable of predicting the
failure pressure for arbitrarily specified loading conditions, has been developed. Also, the
failure types and effects of thermal loading are investigated. In the second part, a
comprehensive FE model has been developed to predict the behavior of the cylinder
subjected to flame impingements. A failure model based on Hashin’s theory has been
implemented to detect various failure modes of the composite. Damage due to resin burn
out and mechanical degradation are also considered in the model. Numerical results are
presented for thermal damage, residual properties and resin content profile of the
cylinder. In the third part, fracture behavior of the cylinder with an axial surface crack in
the liner has been studied using fracture mechanics and a globallocal FE technique with
consideration of autofrettage effect. Results on the fracture parameters (K and Jintegral)
with various autofrettage levels, crack sizes and crack shapes are presented.
v
ACKNOWLEDGMENTS
The author wishes to extend his deepest gratitude to his academic advisor, Dr. K.
Chandrashekhara, for his continued guidance, advice, encouragement and financial
support throughout the course of the investigation and successful completion of this
dissertation research.
The author also wishes to extend his greatest appreciation to the members of the
advisory committee, Dr. Lokeswarappa. R. Dharani, Dr. HaiLung Tsai, Dr. Gregory E.
Hilmas, and Dr. William E. Showalter for their advice and encouragement, and their time
and effort for review of this dissertation.
Many thanks go to Dr. S. Sundararaman for his prior input in this research. The
author also appreciates the assistance from his fellow colleagues and friends, Mr. Jian
Chen, Mr. V.G.K. Menta and Mr. R. Vuppalapati.
The author would like to take this opportunity to thank Mr. William Chernicoff of the
US Department of Transportation for his assistance with information and ideas. The
funding of this research by the US Department of Transportation is gratefully
acknowledged.
The author would also like to acknowledge the financial support received from the
Department of Mechanical and Aerospace Engineering at Missouri S&T for Graduate
Research Assistantship and Graduate Teaching Assistantship.
Finally, the author wishes to express his deepest gratitude to his parents, his sisters
and brothersinlaw for their understanding, patience, encouragement, support, and for
helping realize and accomplish his dreams.
vi
TABLE OF CONTENTS
Page
PUBLICATION DISSERTATION OPTION ................................................................ iii
ABSTRACT ..................................................................................................................iv
ACKNOWLEDGMENTS ..............................................................................................v
LIST OF ILLUSTRATIONS .........................................................................................ix
LIST OF TABLES ........................................................................................................xi
SECTION
1. INTRODUCTION ......................................................................................................1
1.1. BACKGROUND .....................................................................................................1
1.2. SCOPE AND OBJECTIVES ...................................................................................3
1.3. CONCLUDING REMARKS ..................................................................................5
PAPER
I. FAILURE PRESSURE PREDICTION OF COMPOSITE CYLINDERS FOR HYDROGEN STORAGE USING THERMOMECHANICAL ANALYSIS AND NEURAL NETWORK ...........................................................................................7 ABSTRACT ..........................................................................................................7
1. INTRODUCTION .............................................................................................8
2. SHEAR DEFORMABLE SHELL THEORY ...................................................10
3. COMPOSITE FAILURE MODEL ...................................................................13
4. MATERIAL PROPERTIES .............................................................................14
5. FINITE ELEMENT SIMULATION .................................................................15
6. NEURAL NETWORK MODEL ......................................................................17
7. RESULTS AND DISCUSSION .......................................................................19
8. CONCLUSIONS .............................................................................................22
REFERENCES ....................................................................................................23
II. ANALYSIS OF COMPOSITE HYDROGEN STORAGE CYLINDERS SUBJECTED TO LOCALIZED FLAME IMPINGEMENTS ..............................48
ABSTRACT .......................................................................................................48
1. INTRODUCTION ..........................................................................................49
2. MODELING OF HIGH PRESSURE COMPOSITE HYDROGEN STORAGE CYLINDERS ..................................................................................................51
vii
2.1. Thermal Model .........................................................................................51
2.2. Sublaminate Model .................................................................................53
2.3. Formulation of Finite Element Model .......................................................55
3. MATERIAL MODELS ....................................................................................56 3.1. Temperature Dependent Material Properties .............................................56
3.2. Composite Failure Criteria ........................................................................57
3.3. Model for Hydrogen Gas ..........................................................................58
4. FINITE ELEMENT SIMULATION PROCEDURE .........................................59 5. RESULTS AND DISCUSSION .......................................................................60
6. CONCLUSIONS .............................................................................................62 REFERENCES ....................................................................................................63
III. FRACTURE ANALYSIS OF HYDROGEN STORAGE COMPOSITE CYLINDERS WITH LINER CRACK ACCOUNTING FOR AUTOFRETTAGE EFFECT .............................................................................................................88
ABSTRACT .......................................................................................................88
1. INTRODUCTION ...........................................................................................89 2. METHODOLOGY ..........................................................................................91
2.1. Autofrettage Effect on High Pressure Composite Cylinder for Hydrogen Storage .....................................................................................................91
2.2. Stress Intensity Factor (K) Evaluation .......................................................93
2.3. JIntegral Evaluation ................................................................................94
2.4. Material Models ........................................................................................95
3. FINITE ELEMENT SIMULATION ...............................................................97 3.1. Global Model ............................................................................................98
3.2. Local Model .............................................................................................99
3.3. Simulation Procedure ..............................................................................100
4. RESULTS AND DISCUSSION .....................................................................101 4.1. Autofrettage Process Simulation ............................................................101
4.2. Stress Intensity Factor (K) and Jintegral ...............................................102
4.3. Stress Field Characterization on the Crack Tip Vicinity .........................103
5. CONCLUSIONS ..........................................................................................104
REFERENCES .................................................................................................105
viii
SECTION
BIBLIOGRAPHY .....................................................................................................129
VITA ..........................................................................................................................132
ix
LIST OF ILLUSTRATIONS Figure Page
PAPER I
1. Structure scheme of hydrogen storage cylinder .........................................................34
2. Doubly curved shell and coordinate system ...............................................................35
3. Finite element model of hydrogen cylinder ...............................................................36
4. Feedforward backpropagation Neural Network architecture .....................................37
5(a). Uniform thermal loading with Tin=Tout (in Case 1) ................................................38
5(b). Uniform thermal loading Tin=Tout (in Case 2) .......................................................39
5(c). Uniform thermal loading Tin=Tout (in Case 3) .......................................................40
6(a). Gradient thermal loading with Tout=50oC (in Case 1) ............................................41
6(b). Gradient thermal loading with Tout=50oC (in Case 2) ............................................42
6(c). Gradient thermal loading with Tout=50oC (in Case 3) ............................................43
7. Failure pressure with inside temperature variation (Tout=25oC) ..................................44
8. Plybyply failure predictions under various thermal loadings ...................................45
9(a). Comparison of failure pressures from NNk and ABAQUS at = 15o ...................46
9(b). Comparison of failure pressures from NNk and ABAQUS at = 25o ...................47
PAPER II
1. Schematic of hydrogen cylinder ................................................................................73
2. Curve fitting for hydrogen gas state equation at constant density ...............................74
3. Finite element model of the cylinder .........................................................................75
4. Stacking sequence of the cylinder wall ......................................................................76
5. Finite element implementation schemes ....................................................................77
6. Variation of sink temperature with film coefficient ...................................................78
7. Internal pressure variation with time for various flame area sizes ..............................79
8. Temperature distributions along the length at inner surface of the aluminum liner .....80
9. Temperature distributions through composite thickness ............................................81
10. Residual resin content through the thickness ...........................................................82
11. Stress (S11) distribution through the thickness .........................................................83
12. Stress (S22, S33) distribution through the thickness ...................................................84
13(a). Fiber fracture index (Imt) contour around heat source ..........................................85
x
13(b). Matrix cracking index (Ift) contour around heat source .......................................86
13(c). Density index (ρ/ρ0) contour around heat source .................................................87
PAPER III
1. Schematic of hydrogen composite cylinder .............................................................112
2. Diagram of autofrettage process ..............................................................................113
3. Schematic of domain integral evaluation .................................................................114
4. Global finite element model ....................................................................................115
5. Local finite element model ......................................................................................116
6. Implementation scheme ..........................................................................................117
7. vonMises stress distribution in liner .......................................................................118
8. Cyclic stressstrain curves for various autofrettage levels ........................................119
9. Stress intensity factor (K) along crack front for various autofrettage levels .............120
10. Jintegral along crack front for various autofrettage levels ....................................121
11. Stress intensity factor (K) against pressure loading for various autofrettage levels 122
12. Jintegral against pressure loading for various autofrettage levels ..........................123
13. Stress intensity factor (K) along crack front with various geometric ratios ............124
14. Jintegral along crack front with various geometric ratios ......................................125
15. Stress distribution of the crack front vicinity .........................................................126
16. Transition of plastic zone shapes along crack front ................................................127
17. Plastic zone shapes for various autofrettage levels .................................................128
xi
LIST OF TABLES
Table Page
PAPER I
1. Ultimate strength of carbon/epoxy composite ...........................................................27
2. Mechanical and thermal properties of Sglass/epoxy .................................................28
3. Mechanical and thermal properties of Aluminum Alloy 6061T6 ..............................29
4. Layup configurations for various winding patterns ..................................................30
5. Weights and biases for trained neural network ..........................................................31
6. Scale constants for trained neural network ................................................................32
7. Testing cases and maximum error of prediction ........................................................33
PAPER II
1. Curve fitting parameters for transverse and shear modulus ........................................67
2. Thermal expansion coefficients of carbon/epoxy .......................................................68
3. Specific heat and thermal conductivity of carbon/epoxy ............................................69
4. Parameters for resin reaction model ..........................................................................70
5. Strength of carbon/epoxy ..........................................................................................71
6. Design parameters for the cylinder ............................................................................72
PAPER III
1. Mechanical properties of carbon/epoxy composite ..................................................110
2. Mechanical properties of Aluminum Alloy 7075T651 ...........................................111
1. INTRODUCTION
1.1. BACKGROUND
Currently, the energy crisis and environmental pollution arising from burning fossil
fuel in vehicles are identified as some of the major concerns in the global world.
Hydrogen, a renewable and clean energy resource, is a promising substitute for fossil
fuels. One of the key challenges for the usage of hydrogen gas in automobiles is to
develop a compact and efficient way of hydrogen storage. The solutions for this
challenge can be categorized into three main groups [12]: (a) Cryogenic hydrogen
storage: It provides high volumetric density (0.07 kg/L) and good weight density (2.8 %),
but liquefaction (423.2 oF) is an intensive energy consuming process and evaporation
reduces the gas usage efficiency. (b) Hydrogen storage materials: Traditional metallic
hydrogen storage materials provide a safe way to store hydrogen gas, but a low weight
density (1.4 %) and operation complexity prohibit it from practical applications.
Recently, carbon nanotubes have attracted much research interest as a future hydrogen
storage material, but it still remains in the early investigation phase [3]. (c) Compressed
hydrogen gas: It is expected to be the main stream for hydrogen storage in the near future
as it provides good volumetric and weight density (0.03 kg/L and 6%) and simplicity of
transportation and storage.
Traditionally, compressed hydrogen gas is stored in metallic cylinders (Type I
cylinder). The storage pressure for this type of cylinder is low (usually less than 25 MPa)
and the capacity of hydrogen gas storage is limited. Also, hydrogen embrittlement can
result in microcracks and reduce the strength of the cylinder. The Type II cylinder is
developed by wrapping fiberreinforced composite materials in the hoop direction on the
metallic cylinder [4]. It reduces the weight of the cylinder significantly. However, this
still does not meet the requirement of hydrogen storage capacity for automotives. To
further reduce the weight and increase the storage capacity, fully wrapped composite
cylinders (Type III and Type IV) have been introduced. The cylinders are manufactured
by the filament winding technique. In this process, a liner is used as a mandrel and the
high strength, low density composite (fiber strength 56 GPa, composite density 1.6
g/cm3) is fully wrapped in both the helical and the hoop directions. The helical winding
2
produces helical layers to bear the axial loading, while the hoop winding generates hoop
layers to carry circumferential loading. The liner serves as a gas barrier after the cylinder
is manufactured. The Type III differentiates the Type IV by the material used for the liner
(aluminum for Type III and polymer for Type IV). To obtain efficient storage capacity,
the cylinders are designed for pressures as high as 5,000 to 10,000 psi and, hence, the
failure of the cylinder would lead to a catastrophic accident. In this context, safe
installation and operation of highpressure composite cylinders for hydrogen storage are
of primary concern. To design the cylinder with the highest possible safety, reliability
and minimum weight considerations, mechanics relevant to the behavior of the cylinder
must be well understood.
The early technique used for analyzing filamentwound composite cylinders is netting
analysis [57]. This procedure has been widely used in the industry for its simplicity. A
static equilibrium principle is applied to obtain the stress on the fiber by neglecting the
contribution of the resin matrix. Although this technique provides a concise way to
predetermine some design parameters for cylinder prototypes, more detailed analysis is
necessary for examining and optimizing the high pressure composite cylinder for
hydrogen storage under various operating conditions.
Considering the effect of resin matrix, many studies have been focused on developing
an analytical solution for composite cylinders under various loadings. Lekhnitskii [8] laid
the foundation for analyzing the anisotropic elasticity. Numerous authors [913]
advanced the model for the stress analysis of cylinders under uniaxial, biaxial and
combined centrifugal pressure loadings in terms of stress functions. Later on, based on a
plainstrain assumption, Akcay and Kaynak [14] analyzed closedend cylinders under
uniform thermal loading. Sayman [15] incorporated a general hydrothermal effect in the
model that is suitable for multilayered thin/thick composite cylinders for the axially
symmetric case under uniform or parabolic temperature distributions. Tabakov [16]
developed a model to obtain exact solutions for the thick laminated anisotropic cylinder
with closed ends, but this model was limited to five layers and was not universal. In his
later work [17], a general model was developed by deriving the governing differential
equations instead of stress functions without considering the end effects and closing
3
plates. More recently, Chapelle and Perreux [18] extended the analytical method to
analyzing a Type III hydrogen cylinder by including plastic flow of the liner.
The Finite Element Method (FEM) provides a convenient tool to analyze composite
cylinders with consideration of nonlinearities, failure modes and various loading
conditions. A three dimensional finite element was developed by Hoa et al. [19] for the
strain analysis of fiber reinforced plastic vessels containing discontinuities such as
manhole connections or nozzles. Considering the change of winding angles through the
thickness of helical laminates, finite element analyses were performed by Park et al. [20]
through coding the winding angle to each solid element. Kabir [21] modeled the structure
of the cylinder wall as an elastic, ideally plastic liner, reinforced with quasiisotropic
elastic composite. Tam et al. [22] analyzed the composite tank considering both material
and geometric nonlinearities. Gray and Moser [23] described a method which has been
developed to analyze filamentwound composite pressure vessels accounting for the
highly orthotropic nature of vessel structures. Kim et al. [24] employed a 3D element to
compute stresses for optimizing the composite pressure vessel design. In addition,
significant studies were conducted by several researchers [2528] on the analysis of
composite pressure vessels with incorporating failure and progressive damage models in
FE programs. The fracture and fatigue behavior of composite pipes and cylinders have
also been investigated by many authors [2934] using both stress/strain criteria and direct
crackmodeling techniques in finite element models.
1.2. SCOPE AND OBJECTIVES
Based on the literature survey, many researchers have used finite element method on
the study of composite vessels or pipes, but there is no significant research on the
analysis of Type III cylinders subjected to thermomechanical loading. In the case of fire
impingements, the previous studies have been carried out on flat composite panels and
lack the capability of analyzing composite cylinders considering both mechanical and
thermal damage. Furthermore, fracture failure is another essential factor for the safety
and design lifeexpectancy of the cylinder. Most of the previous studies have performed
fracture analysis either on compressed natural gas cylinders or on pressure vessels used
for aerospace. Intensive analysis has been conducted on metallic cylinders and a few are
4
related to cylinders with a metallic liner wrapped by composites. However, not much
research has been performed on composite hydrogen cylinders with consideration of the
autofrettage effect.
As an effort to develop the finite element model to predict the behavior of Type III
hydrogen cylinders for the safety concern and design guidance, this study focuses on
three aspects. The first one is to develop a finite element model that can predict the
failure pressure of the cylinder subjected to combined thermal and mechanical loadings.
The second one is to develop a comprehensive finite element model that can identify
failure modes of the cylinder when it is attacked by fire impingement. The third one is to
evaluate the performance of the cylinder containing liner cracks from the perspective
view of fracture mechanics using finite element simulation technique.
This dissertation has been prepared in the form of three parts corresponding to the
addressed problems.
The first part is titled “Failure Pressure Prediction of Composite Cylinders for
Hydrogen Storage using Thermomechanical Analysis and Neural Network.” In this
part, a finite element simulation tool for the design of hydrogen storage cylinders has
been developed. The structural response of the cylinder is analyzed using laminated shell
theory accounting for transverse shear deformation and geometric nonlinearity. A
composite failure model is used to evaluate the failure pressure. A backpropagation
Neural Network model is developed based on the results of finite element analysis to
predict the maximum failure pressure for arbitrary thermomechanical loading conditions.
The second part is titled “Analysis of Composite Hydrogen Storage Cylinders
Subjected to Localized Flame Impingements.” In this part, a comprehensive nonlinear
finite element model has been developed for predicting the behavior of composite
hydrogen storage cylinders subjected to high pressure and localized flame impingements.
The model is formulated in an axisymmetric coordinate system and incorporates various
submodels to capture the behavior of the composite cylinder under extreme thermo
mechanical loadings. Submodels are implemented in ABAQUS commercial finite
element code using user subroutines. Numerical results are presented for thermal damage,
residual properties and profile of resin content of the cylinder wall.
5
The third part is titled “Fracture Analysis of Hydrogen Storage Composite
Cylinders with Liner Crack accounting for Autofrettage Effect.” In this part, a
globallocal finite element model is developed to investigate the axial surface flaws in the
liner of high pressure composite cylinders for hydrogen storage using fracture mechanics.
The effect of autofrettage process is studied due to its strong influence on the cylinder
fracture behavior. The autofrettage process simulation is conducted in the global model.
The local model, which is driven by the results of the global model, performs a detailed
analysis of the crack to assure accurate computation of fracture parameters. Results of
both stress intensity factor (K) and Jintegral are reported along the crack front in four
autofrettage levels and with different crack sizes. The plastic zone along the crack front is
also studied.
1.3. CONCLUDING REMARKS
In the first part, a doubly curved shell model accounting for transverse shear
deformation is used for the thermomechanical analysis of hydrogen composite storage
cylinders. Temperature dependent material properties of the load carrying carbon/epoxy
layer and geometry nonlinearity are also considered in the numerical model. Under
uniform thermal loading, a temperature increase significantly raises the maximum failure
pressure based on the TsaiWu failure criterion. Contrastively, the nonuniform thermal
loading can cause an uneven load distribution and hence decrease the maximum failure
pressure. The thickness ratio also plays an important role in determining the maximum
failure pressure and should be selected appropriately based on the thermal and
mechanical loading conditions. A neural network model is developed and used to predict
the failure pressure. The performance of the trained neural network is then evaluated by
comparing the predicted values with those of testing cases. The results are in good
agreement.
In the second part, a comprehensive finite element model has been developed to
analyze composite hydrogen storage cylinders subjected to high pressure and flame
impingements. The model considers the resin reaction, heat exchange between the
hydrogen gas and liner, and the progressive failure process. A sublaminate model has
been developed to reduce computational time. A temperature dependent material model
6
along with a failure model has been developed and implemented to accurately predict
various failure modes for the hydrogen storage cylinder. Analysis of a typical high
pressure composite hydrogen cylinder under fire exposure is conducted by using the
developed models. Parametric studies are done on heat exchange rate (between hydrogen
gas and the liner) and the size of the flame source. Stresses, temperature profile and
failure types are reported. The developed model can be used to accommodate various
types of thermal and mechanical loadings, lamina stacking sequence, and lamina
thickness to establish safe working conditions and design limits for hydrogen storage
cylinders.
In the third part, a globallocal finite element model has been developed to predict the
fracture behavior of high pressure composite cylinders for hydrogen storage. Simulation
of the autofrettage process is carried out in the global model. Plastic hardening and the
Bauschinger effect are observed in the results. Both stress intensity factor (K) and J
integral are computed along the crack front in the local model with consideration of
autofrettage influence and crack size effect. It is found that the autofrettage process
significantly improves the cylinder fracture performance and the smaller crack size
reduces the value of fracture parameters dramatically. The plastic zone around the crack
tip is studied in terms of shape and size. The fracture behavior is discussed through
observation of the plastic zone and the corresponding selection of parametric
characterization is suggested.
The current research can be extended in several ways for future work. The developed
Neural Network model for failure pressure prediction can be applied to optimization of
composite layups under arbitrary environmental temperature conditions. The second part
of the model can be extended to multiphysics analysis by simulating the fluid field of
hydrogen gas in the cylinder. Pressure release device can be designed based on the
prediction of simulation to minimize the hazard of cylinder failure when subjected to
accidental fire. The fracture model can be used as a tool for cylinder autofrettage process
to obtain an optimum stress state to restrict crack growth in the liner. Also, the currently
developed fracture model can be extended to predict the fatigue life of the cylinder and
provide guidance for material selection and layup optimization of the composite wall to
achieve premium fracture performance.
7
PAPER I:
FAILURE PRESSURE PREDICTION OF COMPOSITE CYLINDERS FOR
HYDROGEN STORAGE USING THERMOMECHANICAL ANALYSIS AND
NEURAL NETWORK
ABSTRACT
Safe installation and operation of highpressure composite cylinders for hydrogen
storage are of primary concern. It is unavoidable for the cylinders to experience
temperature variation, and significant thermal input (or flux) during the service. The
maximum failure pressure that the cylinder can sustain must be affected due to the nature
of temperature dependent composites, integrity of the matrix and fibers and complexity
of the cylinder design. Most of the analysis reported in highpressure composite cylinders
is based on simplified assumptions and does not account for complexities like thermo
mechanical behavior and temperature dependent material properties. In the present work,
a comprehensive finite element simulation tool for the design of a hydrogen storage
cylinder is developed. The structural response of the cylinder is analyzed using laminated
shell theory accounting for transverse shear deformation and geometric nonlinearity. A
composite failure model is used to evaluate the failure pressure under various thermo
mechanical loadings. A backpropagation Neural Network (NNk) model is developed to
predict the maximum failure pressure using the analysis results. The failure pressures
predicted from the NNk model are compared with those from testing cases. The
developed NNk model is capable of predicting the failure pressure for any given loading
condition.
8
1. INTRODUCTION
Composite highpressure cylinders have potential application as hydrogen storage
systems in automotive, transportation, portable, and stationary storage systems due to
their light weight, simplicity of the storage and low cost for storage and transport of
hydrogen gas [1]. Typically, a composite highpressure cylinder is made of a high
molecular weight polymer or aluminum liner that serves as a hydrogen gas permeation
barrier. A filamentwound, carbon/epoxy composite laminate overwrapped outside of
the liner provides the desired pressure load bearing capacity [2]. A vehicle fuel system
cylinder is capable of sustaining pressures of 5,000 psi or higher by taking advantage of
the high strength and low specific weight of modern high performance composites. In
addition, the maturation of the filament winding manufacturing process further reduces
the price to being practical and common for use in mass transportation systems.
To design composite highpressure cylinders with the highest possible safety,
reliability and minimum weight considerations, the behavior of composite structures
under various mechanical and thermal loadings, including localized and nonlocalized
flames, needs to be well understood. Studies have been conducted by various researchers
[35] on the structure of hydrogen composite cylinders under mechanical loadings. Using
finite element method as a powerful numerical tool, numerous studies have been
conducted on highpressure cylinder analysis [68]. Compared to pure mechanical
loading, fewer studies have been conducted on hydrogen composite cylinders subjected
to thermal loads and combined thermomechanical loads [9, 10].
In the present study, a thermomechanical finite element model has been developed
for the analysis of hydrogen storage cylinders. The composite laminate wall of hydrogen
9
composite cylinder typically consists of helical and hoop laminated layers. Both these
layers, along with an aluminum liner, are considered for the analysis. During service,
hydrogen composite cylinders unavoidably experience various thermal loadings
combined with high inner pressure. To account for working temperature variation in the
service, uniform temperature loadings ranging from 25C to 140 C are considered for the
analysis, above which the matrix begins to burn. During the gas filling process, the inner
temperature can go up to around 100 C [10]. Hence, nonuniform thermal loadings have
also been included in the study. The variation of material properties with temperature is
significant for most composites. A temperature dependent material model has been
developed and implemented in commercial finite element code ABAQUS, using user
subroutines. A laminated shell theory [11, 12] accounting for outofplane shear strains
and geometric nonlinearity is used for the analysis.
When considering the combination of various thermal loadings, winding angles and
lay up configurations in the analysis, it is a tremendous task to optimize the cylinder
design and predict maximum failure pressure through casebycase simulation. A back
propagation Neural Network (NNk) model is then developed to predict the failure
pressure using the results from a few typical finite element simulation cases. The training
process consists of training the network with three sets of simulation results with various
winding angles and thermal loadings. Once trained, the developed NNk model can be
used for guidance and optimization of hydrogen cylinder design. Some testing cases,
which are not included in the training sets, are utilized to compare with the predicted
failure pressure from the NNk model. A good agreement is found between failure
pressures from testing cases and NNk model prediction.
10
2. SHEAR DEFORMABLE SHELL THEORY
A schematic of a hydrogen composite cylinder wall is shown in Figure 1. The inner
liner is made of high molecular weight polymer or aluminum that serves as a hydrogen
gas permeation barrier. A filamentwound, carbon/epoxy composite laminate over
wrapped on the outside of the liner provides the desired pressure load bearing capacity
[13]. In many current designs, a glass/epoxy layer is placed over the carbon/epoxy
laminate to provide impact and damage resistance. The doubly curved shell theory
accounting for out of plane shear deformations and geometric nonlinearity is used for the
analysis of composite hydrogen storage cylinders.
A multilayered doubly curved shell is shown in Figure 2. The curved coordinated
system 1 2, , is used in space description. The coordinates 1 and 2 specify the
position on the middle surface, while measures the distance, along the outward normal,
from the midsurface to an arbitrary point on the shell. The displacement field can be
written as:
o1 2 1 2 1 1 21
u( , , ) = (1 + ) ( , ) + ( , )uR (1.a)
o1 2 1 2 2 1 22
v( , , ) = (1 + ) ( , ) + ( , )vR (1.b)
o1 2 1 2w ( , , ) = ( , )w (1.c)
The nonlinear straindisplacement relations based on Sanders’s shell theory can be given
as:
o o= =x yx x y y + ζ ; + ζ ε ε ε εκ κ
o o o= = =xyxy xy yz yz xz xz + ζ ; ; γ γ γ γ γ γκ (2)
11
where 0j jε and κ are defined as:
2
o o oo 1xx 2
11 111 1 1
1 1 1u w w = + + ; = ε κ2αξ ξ ξα αR
2
oo 0 0 2y y2
2 2 2 2 2 22
v w1 1 1w+ ; κε α R 2α αξ
o o o o oxy
1 2 1 21 2 1 2
1 1 1v u w w = + + γα α 2α αξ ξ ξ ξ
; o o o2yz
22 2
1 w v = +  γξα R
(3)
o o o1xz
11 1
1 w u = +  γξα R
o o2 1xy o
1 2 1 21 2 1 2
1 1 1 1v u = +   cκξ ξ ξ ξα α α α
0 1 1 2 21 2
1 1 1c =  ; dx = α dξ ; dy = α dξ2 R R
In Eq. (3), u and v are the displacements in the direction of the tangents to the coordinate
lines 1 and 2 , respectively, w is the displacement in the direction of the outward
normal and 1 and 2 are the rotations.
The stressstrain relation, accounting for thermal effects, in the shell coordinates for a
k th layer can be expressed as [12]:
11 12 16
12 22 26
16 26 66
44 45
45 55
0 00 00 0
0 0 00 0 0
x x x
y y y
xy xy xy
yz yz
xz xzk k k
Q Q Q ε TQ Q Q ε TQ Q Q T
Q QQ Q
(4)
where ijQ are the transformed elastic coefficients, T is the given temperature distribution,
and xyyx ,, are the thermal expansion coefficients in the shell coordinates.
12
The laminate constitutive equations can be obtained by integrating Eq. (4) over the
thickness, and is written as:
x 11 12 16 11 12 16
y 12 22 26 12 22 26
xy 16 26 66 16 26 66
xz 44 45
yz 45 55
x 11 12 16 11 12 16
y 12 22 26 12 22 26
xy 16 26 66 16 26 66
N A A A 0 0 B B BN A A A 0 0 B B BN A A A 0 0 B B BQ 0 0 0 A A 0 0 0
Q 0 0 0 A A 0 0 0M B B B 0 0 D D DM B B B 0 0 D D DM B B B 0 0 D D D
0 Tx x0 Ty y0 Txy xy0xz0yz
Tx x
Ty y
Txy xy
ε Nε Nγ Nγ 0
 γ 0κ Mκ Mκ M
(5)
where TN and TM are thermal stress and moment resultants
/ 2 2
/ 21
h
ij ij ij ijhA B D Q z z dz
, 1,2,6i j (6.a)
/ 2
/ 2
h
ij i j ijhA K K Q dz
, 4,5i j (6.b)
11 12 16
/ 2
12 22 26/ 2
16 26 66
,, 1,,
T Tx x x
hT Ty y yhT Txy xy xy
N M Q Q QN M Q Q Q z TdzN M Q Q Q
(6.c)
where K is a shear correction factor.
Following the standard finite element procedure, the generalized displacements in any
element are given by:
1
1 1
2 2
N
ii
i
u uv vw w
(7)
where N is the number of nodes in the element and i are the interpolation functions.
Substituting Eq. (7) in Eq. (3), the strains can be expressed as:
13
1 2 3 ; ;B B B (8)
The finite element equation is written as:
e e e eTK F F (9)
where ,
1 1 1 2 2 1 2 2 3 3 ( )e T T T T TK B AB B BB B BB B DB B SB d Area
1 2
Te u v w
1 2 ( )e T TF B N B M d Area
1 2 ( )e T T T TTF B N B M d Area
For any given mechanical and temperature loadings, Eq. (9) can be assembled and solved
to determine displacements and stresses.
3. COMPOSITE FAILURE MODEL
The TsaiWu failure criterion is used for failure evaluation of hydrogen composite
storage cylinders [14]. Taking 1 as the fiber direction and 2 and 3 as transverse
directions, the TsaiWu failure criterion can be expressed as:
0.1 2 221112
21266
21355
22344
22222
21111222111
FFFFFFFFI F (10)
The coefficients in Eq. (10) are defined as:
11 1
t c
FX X
, 21 1
t c
FY Y
, 111
t c
FX X
,
221
t c
FYY
, 223
441
SF , 2
1355
1S
F , 212
661
SF ,
14
212 2
1 1 1 1 1 1 112 biax biax
biax t c t c t c t c
FX X Y Y X X YY
or
12 11 22F f F F ( 1 1f )
where, tX and cX are tensile and compressive stress strengths along the fiber direction,
tY and cY are tensile and compressive stress strengths in the transverse fiber direction,
23S , 13S and 12S are the maximum shear strengths in corresponding planes, biax is the
equibiaxial stress at failure and f is an experience coefficient.
4. MATERIAL PROPERTIES
Mechanical and thermal properties of fiber reinforced composites vary significantly
with temperature. As the carbon/epoxy laminate carries the pressure loading from the
hydrogen gas, the effect of temperature on its material properties cannot be ignored. The
moduli and thermal expansion coefficients are dependent on temperature. For HFG
CU125 carbon/epoxy, the temperature dependent material properties are given by [15]:
E1= 0.066 T + 128 (GPa) (25C < T < 140C)
E2 = 0.064 T + 10.67 (GPa) (25C < T < 140C)
G12 = 0.034 T + 5.39 (GPa) (25C < T < 140C) (11)
12 = 0.0005 T + 0.44 (25C < T < 140C)
α1= (0.0003 T2 0.04 T + 2.09) × 106 (25C < T < 140C)
α2 = (0.0041 T2 0.23 T + 32.2) ×106 (25C < T < 140C)
15
Furthermore, G13 is taken as G12, and G23 is assumed as 0.7G12. The ultimate
strengths of carbon/epoxy do not change much with this temperature range and are
assumed to be constant and are listed in Table 1. The material properties for glass/epoxy
are listed in Table 2. The outer most glass/epoxy layer is primarily used for protection of
the load bearing carbon/epoxy lamina. Hence temperature dependent material properties
are not used for the glass/epoxy layers. Properties of the innermost aluminum liner are
listed in Table 3.
5. FINITE ELEMENT SIMULATION
ABAQUS is an integrated and openended Finite Element Analysis code, which is
widely used by the industry as well as researchers for the flexibility of implementing user
defined subroutines and its powerful nonlinear solver. With those features, the user
defined problem can be built up by combination of the basic frames provided by the
ABAQUS code and user model specialties implementing subroutines. All the modeling
features described in this work have been thus implemented in this code. A laminated
shell element, based on doubly curved shell theory, accounting for membrane, bending
and membranebending coupling and transverse shear effects, is suitable for modeling
both thin and thick laminated composites. For this purpose, the laminated composite wall
of the cylinder is modeled by using a doubly curved 8node shell element (S8R). In order
to estimate the failure pressure of the cylinder, it is necessary to include a failure
criterion. TsaiWu failure theory is utilized to check and report the plybyply laminate
failure by using a user subroutine UVARM. In addition, the temperature dependent
material properties are incorporated in the model by using subroutine USDFLD so that, at
16
each integration point, the material properties are determined by the given temperature.
The orientation of each element at every ply is handled by subroutine ORIENT according
to the winding pattern. The cylinder is modeled and meshed using the ABAQUS/CAE
preprocessor as shown in Figure 3. Due to the symmetry, 1/8th of the cylinder is
considered for the analysis. The comprehensive model is then solved by using the
ABAQUS/standard solver with geometric nonlinearity considered.
The dimensions considered in the present cylinder analysis are based on a typical
design from the literature [13]. The outer radius of the cylinder is taken as outR = 0.25 m
and the inner radius inR = 0.22 m (Figure 1). The pressure bearing carbon/epoxy laminate
consists of 24 plies resulting in a composite shell of thickness 28 mm. The protective
glass/epoxy layer and liner are 2 mm and 2.5 mm thick respectively. The cylinder is
subjected to an internal pressure that gradually increases until failure occurs in the first
ply. To manufacture closed cylinders, two types of winding patterns are usually used:
hoop and helical/polar windings. The thickness ratio R (total thickness of helical
laminate/total thickness of hoop laminate) affects the failure pressure of the cylinder and
a range of 0.1 to 2.0 is studied. The winding angle of laminae also affects the failure
pressure of the cylinder and a range of 10◦ to 30◦ for helical winding and 89o for hoop
winding has been considered based on manufacturing feasibility. The plies in the
protection laminate are oriented as 45 angle ply.
17
6. NEURAL NETWORK MODEL
A feedforward backpropagation Neural Network (NNk) is used to predict the failure
pressure of a hydrogen cylinder. A schematic of the NNk is shown in Figure 4. The
relationship of failure pressure and the inputs (thickness ratio R , temperature inside the
cylinder inT , temperature outside the cylinder outT , and winding angle ) is modeled by a
twolayer (hidden layer and output layer) network. Each layer consists of a number of
processing units, with an activation function, known as neurons. For faster training and
robust NNk, inputs are scaled to a desirable range by a designed transfer function Tinf
before entering the input layer. Inputs are passed through weighted connections to the
hidden layer and then to the output layer. The output P is, finally, scaled back to failure
pressure P by a designed transfer function Toutf . The number of neurons in the hidden
layer and the characterizing weights and biases in the model are determined by training
the NNk.
The input transfer function
( )Tin i i i if I I a b (12)
where
iI are input variables ( 1,2,3and 4i corresponding to , ,in outR T T and respectively)
max minmax mini
i i
n naI I
min { }i i ib n Min a I
[ minn maxn ] is the desired scale range and is taken as [1 1]
and iI
are input training pattern vectors.
18
Normalized input variables iI are given by
( )Ti in iI f I (13)
The activation function in the hidden layer is the Logsigmoid function
1( )1
hxf x
e
(14)
The activation function in the output layer is the Pureline function
( )of x x (15)
The normalized failure pressure P is given by [16]
4
11 1
No h h h oj ji i j
j iP W f W I b b
(16)
where
N is number of neurons in the hidden layer
1ojW are weights in the output layer
hjiW are weights in the hidden layer
ob is bias in the output layer
and hjb are biases in the hidden layer
The output transfer function
( ) /Tout if I P b a (17)
where
max minmax min
n naP P
, 1, 2,3,and 4i
min { }ub n Min a P
, 1, 2,3,and 4i
19
and P
is the output training pattern vector.
The final failure pressure P is given by
( )ToutP f P (18)
Training consists of providing a set of known inputoutput pairs (or patterns) to the
network. Backpropagation learning process has two passes through the network: a
forward calculation pass and an error backpropagation pass. In the forward pass, input
patterns broadcast from input layer to output layer in order to generate the actual results
of network. During the backward propagation, weights in each node are iteratively
adjusted based on the errors using the gradient descent equations. The procedure is
repeated until convergence is achieved. In this study, the inputoutput sets are obtained
from simulation results. The model is trained in MATLAB NNk tool box. The fast
training LevenbergMarquardt Algorithm is adopted in the training process.
7. RESULTS AND DISCUSSION
Five configurations of helical and hoop laminas shown in Table 4 are investigated in
this study. Case studies are conducted on composite cylinders with various thermal
loadings and layup patterns. Failure pressures as a function of thickness ratio R under
uniform thermal loadings for Cases 13 are shown in Figures 5(ac) respectively. The rate
of increase in failure pressure is higher at higher temperatures. This reflects the
nonlinearity of thermal expansion coefficients with variation in temperature. For all the
three cases considered, the failure pressure increases with increase in temperature. In
comparison with Cases 2 and 3, the peak failure pressure is slightly higher than that of
Case 1. Similar results are shown in Figures 6(ac) with gradient thermal loading. In
20
comparison with the uniform thermal loadings, the peak failure pressure is not evident for
some of the inner temperatures considered in figure 5(b). In those cases, all hoop laminae
are placed over helical laminae with inner temperature higher than outer temperature.
Then thermal strain, arising from thermal expansion, becomes larger in all helical
laminae which cause hoop laminae to carry most of the axial loadings. Without helical
laminae sustaining major part of the axial loading, the peak pressure then disappears at
lower thickness ratio area. With increasing thickness ratio, the axialload bearing capacity
of the hoop laminae increases thus resulting in the rise in failure pressure. This
phenomenon cannot be observed in Figures 6(bc) because the helical and hoop laminae
are laid alternatively. From Figures 6(ac), with inner temperature increasing (from 25oC
to 140oC), the failure pressure rises till it reaches the set temperature (50oC) of outside
wall, and then starts to decrease. Also it can be observed that the failure pressure
decreases as the gradient of the nonuniform temperature increases.
By comparison of Cases 1, 2 and 3, the alternative lay up pattern (in Cases 2 and 3)
can result in higher failure pressure than that of nonalternative lay up (in Case 1), when
cylinder is experiencing uniform thermal loading and no significant increase is observed
in gradient thermal loading. However, in Case 1, the location of peak pressure varies a lot
in comparison with that of Cases 2 and 3 under gradient thermal loading. This large
variation might bring down the failure pressure at optimum thickness ratio when
considering various thermal loadings in design. There is no significant difference that can
be observed between Case 2 (constant winding angle in helical laminate) and Case 3
(gradually increased winding angle in helical laminate). To study the effect of helical
winding angle pattern on failure pressure, Cases 2, 4 and 5 ( o o6[±20 /±89 ] ,
21
o o6[±10 /±89 ] and o o
6[±30 /±89 ] ) are compared with different thickness ratios (R) as
shown in Figure 7. For the same thickness ratio, higher peak failure pressure is observed
for smaller winding angle.
Figure 8 shows the TsaiWu failure indicator for each helical and hoop ply in Case 2
for thickness ratio, R=0.5. Curves 1 and 2 (T2525 and T140140 respectively) illustrate
the ply failure under uniform thermal loadings while curves 3 and 4 (T25100 and T100
25 respectively) show the failure under gradient thermal loadings (T2525 implies
Tin=25oC and Tout = 25oC). With uniform thermal loading at 140oC, the curve is observed
to be flat, which implies that all the helical and hoop laminae fail simultaneously.
However, at uniform thermal loading of 25oC, the helical laminae tend to fail first. When
subjected to nonuniform thermal loading, a large slope is observed in the curves. The
inner layers fail first for T25100 ( inT = 25oC and outT =100oC), while the outer layers fail
for T10025 ( inT = 100oC and outT =25oC). This asynchronous behavior of inner or outer
layers during failure must cause a significant drop in maximum failure pressure,
assuming that the cylinder fails when any one of the laminae fails.
The network is trained by using the simulation results from Cases 2, 4 and 5 shown in
Table 4. There are 12 neurons used in the neural network (NNk) model and the training
ratio is set to 0.01. After the network gets converged, the model parameters are obtained
and are listed in Tables 5 and 6. The network model is then capable of predicting the
failure pressure by providing the network inputs ( R , inT , outT and ). To evaluate the
performance of NNk prediction, six testing cases (shown in Table 7) are studied. The
testing data from ABAQUS simulation results, for winding angles not used before (15o
and 25o), are used to compare the predicted results from the trained neural network. The
22
performance of the NNk is then illustrated in Figures 9(ab), and the maximum errors are
reported for each case in Table 7. It can be seen that the simulation results are in good
agreement with the results predicted by the NNk model. The trained network can,
therefore, be used to predict any failure pressure within the trained ranges of temperature,
winding angle and thickness ratio.
8. CONCLUSIONS
A doubly curved shell model accounting for transverse shear deformation is used for
thermomechanical analysis of hydrogen composite storage cylinders. Temperature
dependent material properties of the load carrying carbon/epoxy layer and geometric
nonlinearity are also considered in the numerical model. Five typical cases have been
considered and the analysis is carried out by applying uniform/nonuniform thermal
loading and internal pressure loading. The TsaiWu failure criterion is employed to
predict the failure pressure by checking the failure, layer by layer. Under uniform thermal
loading, a temperature increase significantly increases the maximum failure pressure.
Contrastively, the nonuniform thermal loading can cause an uneven load distribution and
hence decrease the maximum failure pressure. The thickness ratio also plays an important
role in determining the maximum failure pressure and should be selected appropriately
based on the thermal and mechanical loading conditions. A neural network (NNk) model
is developed and used to predict the failure pressures. The performance of the trained
neural network is then evaluated by comparing the predicted values with those of testing
cases and the results are in good agreement.
23
REFERENCES
[1] N. Takeichia, H. Senoha, T. Yokotab, H. Tsurutab, K. Hamadab, H. Takeshitac, H. Tanakaa, T. Kiyobayashia, T. Takanod and N. Kuriyamaa, “Hybrid Hydrogen Storage Vessel, A Novel Highpressure Hydrogen Storage Vessel Combined with Hydrogen Storage Material,” International Journal of Hydrogen Energy, Vol. 28, pp. 11211129, 2003.
[2] C. Liang, H. Chen and C. Wang, “Optimum Design of Dome Contour for Filamentwound Composite Pressure Vessels Based on a Shape Factor,” Composite Structures, Vol. 58, pp. 469482, 2002.
[3] V. V. Vasiliev, A. A. Krikanov and A. F. Razin, “New Generation of Filamentwound Composite Pressure Vessels for Commercial Applications,” Composite Structures, Vol. 62, pp. 449459, 2003.
[4] P. Y. Tabakov and E. B. Summers, “Layup Optimization of Multilayered Anisotropic Cylinders Based on a 3D Elasticity Solution,” Computers and Structures, Vol. 84, pp. 374384, 2006.
[5] J. Park, C. Hong, C. Kim and C. Kim, “Analysis of Filament Wound Composite Structures Considering the Change of Winding Angles Through the Thickness Direction,” Composite Structures, Vol. 55, pp. 6371, 2002.
[6] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247255, 2000.
[7] D. L. Gray and D. J. Moser “Finite Element Analysis of a Composite Overwrapped Pressure Vessel,” 40th AIAA/ASME/SAE/ASEE Joint Propulsion Conference and Exhibit, Fort Lauderdale, FL, AIAA 20043506, pp.115, July 1114, 2004.
[8] I. H. Akcay and I. Kaynak, “Analysis of Multilayered Composite Cylinders under Thermal Loading,” Journal of Reinforced Plastics and Composites, Vol. 24, pp.11691179, 2005.
[9] O. Sayman, “Analysis of Multilayered Composite Cylinders under Hygrothermal Loading,” Composites: Part A, Vol. 36, pp. 923933, 2005.
[10] J. M. Schneider, “Gaseous Hydrogen Station Test Apparatus: Verification of Hydrogen Dispenser Performance Utilizing Vehicle Representative Test Cylinders,” SAE World Congress & Exhibition, Detroit, MI, pp.110, April 2005.
24
[11] K. Chandrashekhara and A. Bhimaraddi, “Thermal Stress Analysis of Laminated Doubly Curved Shells using a Shear Flexible Finite Element,” Computers and Structures, Vol. 52, pp. 10231030, 1994.
[12] K. Chandrashekhara and T. Schroeder, “Nonlinear Impact Analysis of Laminated Cylindrical and Doubly Curved Shells,” Journal of Composite Materials, Vol. 29, pp. 21602179, 1995.
[13] F. Mitlitsky, A. H. Weisberg and B. Myers, “Vehicular Hydrogen Storage Using Lightweight Tanks,” Proceedings of the U.S. DOE Hydrogen Program Review NREL/CP57028890, 2000.
[14] S. W. Tsai and E. M. Wu, “A General Theory of Strength for Anisotropic Materials,” Journal of Composite Materials, Vol. 5, pp. 5880, 1971.
[15] K. J. Yoon and J. Kim, “Prediction of Thermal Expansion Properties of Carbon/Epoxy Laminae for Temperature Variation,” Journal of Composite Materials, Vol.34, pp. 90100, 2000.
[16] M. T. Valoor and K. Chandrashekhara, “A Thick Composite Beam Mode for Delamination Prediction by the Use of Neural Networks,” Composite Science and Technology, Vol.60, pp. 17731779, 2000.
25
LIST OF TABLES
Table 1 Ultimate strength of carbon/epoxy composite
Table 2 Mechanical and thermal properties of Sglass/epoxy
Table 3 Mechanical and thermal properties of Aluminum Alloy 6061T6
Table 4 Layup configurations for various winding patterns
Table 5 Weights and biases for trained neural network
Table 6 Scale constants for trained neural network
Table 7 Testing cases and maximum error of prediction
26
LIST OF FIGURES
Figure 1 Structure scheme of hydrogen storage cylinder
Figure 2 Doubly curved shell and coordinate system
Figure 3 Finite element model of hydrogen cylinder
Figure 4 Feedforward backpropagation Neural Network architecture
Figure 5(a) Uniform thermal loading with Tin=Tout (in Case 1)
Figure 5(b) Uniform thermal loading Tin=Tout (in Case 2)
Figure 5(c) Uniform thermal loading Tin=Tout (in Case 3)
Figure 6(a) Gradient thermal loading with Tout=50oC (in Case 1)
Figure 6(b) Gradient thermal loading with Tout=50oC (in Case 2)
Figure 6(c) Gradient thermal loading with Tout=50oC (in Case 3)
Figure 7 Failure pressure with inside temperature variation (Tout=25oC)
Figure 8 Plybyply failure predictions under various thermal loadings
Figure 9(a) Comparison of failure pressures from NNk and ABAQUS at = 15o
Figure 9(b) Comparison of failure pressures from NNk and ABAQUS at = 25o
27
Table 1 Ultimate strength of carbon/epoxy composite
t
LF cLF t
TF cTF S
LTF Strength
(MPa) 1070 1070 40 170 70
28
Table 2 Mechanical and thermal properties of Sglass/epoxy
E1 (GPa) E2 (GPa) G12 = G13
(GPa)
G23
(GPa) 12 1 (1/◦C) 2 (1/◦C)
55 16 7.6 5.0 0.28 6.3 ×106 32 ×106 t
LF cLF t
TF cTF S
LTF Strength
(MPa) 1620 690 40 140 60
29
Table 3 Mechanical and thermal properties of Aluminum Alloy 6061T6
Elastic modulus, E Poisson’s ratio, Yield strength, y (1/◦C)
70 GPa 0.33 455 MPa 24.3 ×106
30
Table 4 Layup configurations for various winding patterns
Case No. Layup pattern Description
1 o o3s 3s[±20 ] /[±89 ]
2 o o6[±20 /±89 ]
3
o o o o o o
o o o o o o
[±10 /±89 /±14 /±89 /±18 /±89 /±22 /±89 /±26 /±89 /±30 /±89 ]
4 o o6[±10 /±89 ]
5 o o6[±30 /±89 ]
24 layers with total
thickness of 28 mm
Tin=[25 50 75 100 120
140] oC
Tout=[25 50 75 100
120 140] oC
31
Table 5 Weights and biases for trained neural network
Weights in hidden layer Biases
j 1hjW 2
hjW 3
hjW 4
hjW
Weights in
output
layer, 1ojW
hjb ob
1 1.0803 0.1725 1.7439 0.3099 54.4500 6.1185
2 0.3894 0.2582 0.1213 0.5764 123.692 3.6584
3 0.4838 0.3915 0.1974 0.8114 36.1329 3.0100
4 0.0004 1.4978 3.5075 0.0280 26.9054 3.3369
5 0.0197 1.8098 3.9087 0.0127 19.1409 3.1452
6 8.3694 1.6462 1.4688 0.0064 0.3018 7.8153
7 0.3793 0.6444 0.6923 0.7765 1.7120 0.0646
8 1.4274 3.7237 11.3865 0.3180 45.0033 4.3089
9 0.4287 11.4817 10.7445 0.6810 0.3312 1.5414
10 11.3451 0.0102 0.3561 0.8548 0.6626 11.8876
11 1.7027 0.2808 1.7533 0.2670 46.5796 6.7410
12 1.4200 3.7174 11.3598 0.3166 45.1670 4.3021
76.65
32
Table 6 Scale constants for trained neural network
i ia ib a b
1 1.05263 1.10526
2 0.01739 1.43478
3 0.01739 1.43478
4 0.10000 2.00000
0.05090
1.96068
33
Table 7 Testing cases and maximum error of prediction
Inputs Testing
case Tin (oC) Tout (oC) θ (Degree)
Max. Error
(%)
1 40 40 15 1.32
2 30 80 15 1.54
3 130 40 15 1.23
4 40 40 25 1.11
5 30 80 25 2.40
6 130 40 25 1.00
34
Figure 1 Structure scheme of hydrogen storage cylinder
0Carbon/Epoxy 1: 10
0Carbon/Epoxy 2:10
0Glass/Epoxy 26:450Glass/Epoxy 25: 45
0Carbon/Epoxy 23:89
0Carbon/Epoxy 24: 89
Aluminum
Pressure inR
outRoutT
inT
35
Figure 2 Doubly curved shell and coordinate system
36
Figure 3 Finite element model of hydrogen cylinder
37
Figure 4 Feedforward backpropagation Neural Network architecture
R
inT
outT
P
1hb
2hb
hNb
hf
hf
hf
of ToutfT
inf
ob
R
inT
outT
P
11hW
11oW
12oW
1oNW
4h
NW
Input layer Hidden layer Output layer
38
Figure 5(a) Uniform thermal loading with Tin=Tout (in Case 1)
39
Figure 5(b) Uniform thermal loading Tin=Tout (in Case 2)
40
Figure 5(c) Uniform thermal loading Tin=Tout (in Case 3)
41
Figure 6(a) Gradient thermal loading with Tout=50oC (in Case 1)
42
Figure 6(b) Gradient thermal loading with Tout=50oC (in Case 2)
43
Figure 6(c) Gradient thermal loading with Tout=50oC (in Case 3)
44
Figure 7 Failure pressure with inside temperature variation (Tout=25oC)
45
1 3 5 7 9 1113 15 1719 21 230
0.10.20.30.40.50.60.70.80.9
1
Layer Number
Indi
cato
r for
Fai
lure
(IF)
T2525T140140T25100T10025
Figure 8 Plybyply failure predictions under various thermal loadings
46
Figure 9(a) Comparison of failure pressures from NNk and ABAQUS at = 15o
47
Figure 9(b) Comparison of failure pressures from NNk and ABAQUS at = 25o
48
PAPER II:
ANALYSIS OF COMPOSITE HYDROGEN STORAGE CYLINDERS
SUBJECTED TO LOCALIZED FLAME IMPINGEMENTS
ABSTRACT
A comprehensive nonlinear finite element model is developed for predicting the
behavior of composite hydrogen storage cylinders subjected to high pressure and
localized flame impingements. The model is formulated in an axisymmetric coordinate
system and incorporates various submodels to describe the behavior of the composite
cylinder under extreme thermomechanical loadings. A heat transfer submodel is
employed to predict the temperature evolution of the composite cylinder wall and
accounts for heat transport due to decomposition and mass loss. A composite
decomposition submodel described by Arrhenius’s law is implemented to predict the
residual resin content of the thermal damaged area. A submodel for material degradation
is implemented to account for the loss of mechanical properties. A progressive failure
model is adopted to detect various types of mechanical failure. These submodels are
implemented in ABAQUS commercial finite element code using user subroutines.
Numerical results are presented for thermal damage, residual properties and the profile of
the resin content in the cylinder. The developed model provides a useful tool for safe
design and structural assessment of high pressure composite hydrogen storage cylinders.
49
1. INTRODUCTION
High pressure composite cylinders for hydrogen storage are typically made with a
high molecular weight polymer or aluminum liner that serves as a hydrogen gas
permeation barrier. A filamentwound, carbon/epoxy composite laminate overwrapped
on the outside of the liner provides the desired pressure load bearing capacity. Due to the
flammable nature of polymerreinforced composites, there is a high risk of failure of the
composite hydrogen storage cylinder under accidental fire exposure. As the stiffness and
strength of composites are temperature dependent, the high pressure (usually 34.5 MPa to
70.0 MPa) in the cylinder can result in catastrophic failure. Therefore, assessment of
structural integrity of high pressure composite hydrogen storage cylinders subjected to
fire exposure is necessary for safe cylinder design.
Many investigations have been conducted by various researchers [14] on the
behavior of high pressure composite cylinders under mechanical loadings. Using finite
element methods, numerous studies have been performed on highpressure vessel
analysis [57]. Compared to pure mechanical loading and pure thermal loading, there
have been few studies on the composite cylinders subjected to the combined thermal and
mechanical loads [89]. However, those models only consider the temperature range
before composite decomposition occurs and fall short of providing capability to assess
the behavior of cylinders subjected to fire impingement. To study fire effect on
composites, different onedimensional thermal models have been developed to predict the
temperature and the residual resin content as a function of time [1012]. These models
account for heat transfer by conduction, resin decomposition, and the cooling effect of
volatile products passing through the laminate. Therefore, to characterize the fire
50
response of high pressure hydrogen composite cylinders, mechanisms of mechanical
effect, thermal effect and decomposition have to be considered.
In this paper, a coupled thermomechanical finite element model has been developed
to simulate composite hydrogen storage cylinders subjected to high pressure and heat flux
on the wall surface. The model is formulated in an axisymmetric coordinate system
which accounts for outofplane stresses and reduces computational cost dramatically.
When the polymer materials are exposed to a sufficiently high temperature (200300°C),
decomposition reactions and thermochemical expansion begin to occur and the resin
system degrades to form gaseous products and carbonaceous char. In order to incorporate
this phenomenon, the thermal model is built to account for gas convection and heat
generation due to decomposition in addition to conduction of the composite, convection
and radiation of surface. The fire source is modeled as a constant heat flux throughout the
simulation. The inner pressure of the cylinder is dependent on the temperature of
hydrogen gas which is modeled as a sink temperature. The variation of material
properties with temperature is significant for composites, especially at high temperatures.
A temperature dependent material model has been developed and implemented. Hashin’s
theory is used as a progressive failure criterion to predict different types of failure (matrix
cracking and fiber breakage). These models are developed and implemented in a
commercial finite element code ABAQUS, using user subroutines. A typical high
pressure hydrogen composite cylinder is simulated using the developed model and results
from the parametric study are reported.
51
2. MODELING OF HIGH PRESSURE COMPOSITE HYDROGEN STORAGE
CYLINDERS
A strong sequentially coupled thermalstress analysis approach is implemented for
predicting the behavior of composite hydrogen cylinders subjected to flame
impingements and high internal pressure. At each increment, the temperature profile is
obtained using the thermal and resin reaction models. The temperature field is then
imported to the mechanical model with material damage information from the previous
increment. The pressure of the inner cylinder is updated based on the heat absorption of
hydrogen gas, which is computed from the temperature profile. The thermal and
mechanical models are solved sequentially in each increment. As the wall consists of a
large number of laminae, modeling each lamina will cause extraordinary computational
cost, especially when thermal and damage models are also incorporated. Hence, a
homogenization technique is used to smear several laminae to a sublaminate as in Figure
1. The equivalent moduli of the sublaminate are used in the formulation of the finite
element model.
2.1 Thermal Model
The high temperature will cause resin decomposition of the cylinder composite wall.
The decomposition rate of the resin is usually represented by Arrhenius’s law and can be
expressed as [13]:
exp( / )AA E RTt
(1)
where,
– density
52
t – time
T – temperature
A – preexponential factor
AE – activation energy
R – gas constant
Material constants A and EA are determined using Differential Scanning Calorimetry.
In consideration of the resin reaction, the heat transfer equilibrium equation has to
include resin decomposition energy and vaporous migration energy. Since the dimension
in the thickness direction is much less than that of hoop and axial directions, the vaporous
gas is only assumed to transfer in thickness direction. The axisymmetric heat diffusion
equation can be written as [14]:
1p r r z g pg com g
T T T T TC k k k m C Q h ht r r r r z z r t
(2)
where,
pC – specific heat of the composite
k – thermal conductivity
r – displacement through the thickness
gm – gas mass flux
pgC – specific heat of the gas
Q – heat of decomposition
comh – enthalpy of the composite
gh – enthalpy of hydrogen gas
53
The mass flow direction of the gas generated in the laminate is towards the hot face of
the laminate. The total mass flux of the generated gas at a specific spatial location in the
laminate is the sum of the gas mass flux generated from the inner face to this spatial
location. The gas mass flux at any spatial location can be calculated as:
h
W
r
g htm dr
t (3)
where,
hr – distance from the hot face
Wt – wall thickness of the composite
2.2 Sublaminate Model
The principle of sublaminate (Figure 1) homogenization is based on the assumption
that the inplane strains and the interlaminar stresses through the thickness are constant
[1518]. The lamina stressstrain relationship in a global coordinate can be written as:
ooo oio
ioi iii
C CC C
(4)
where, ooC , oiC and iiC are sub matrices of global stiffness matrix, oiC is the transpose of
oiC , o and i are outofplane and inplane stresses respectively, o and i are outof
plane and inplane strains respectively. represents the term is constant through the
laminate.
Partially inverting Eq. (4) yields:
1 1
1 1o ooo oo oi
i ioi oo oi oo oi ii
C C CC C C C C C
(5)
After averaging, Eq. (5) can be expressed as:
54
o oT
i i
A BB D
(6)
where, 1
1
Nk
ook k
tA Ct
, 1
1
Nk
oo oik k
tB C Ct
, 1
1
Nk
oi oo oi iik k
tD C C C Ct
kt is the thickness of each lamina in the smeared sublaminate and t is the total thickness
of the smeared sublaminate.
Partially inverting Eq. (6) yields the equivalent stiffness matrix eqQ of the sub
laminate as:
1 1
1 1o o
T Ti i
A A BB A B A B D
(7)
The equivalent compliance matrix is given by:
11 1
11 1[ ] [ ]eq ijT T
A A BQ SB A B A B D
(8)
Equivalent engineering properties used for the simulation can be obtained from Eq.
(8) as:
11 441/E S , 22 551/E S , 33 111/E S
12 661/G S , 13 331/G S , 23 221/G S (9)
12 45 44/v S S , 13 14 44/v S S , 23 15 55/v S S
After the global stresses and strains of the sublaminates are obtained, the stresses in
each lamina are obtained in the global material coordinates as:
o ok
Ti o ik kk
B D
(10)
where k is the thk lamina of the sublaminate.
55
Finally, the stresses in the local material coordinate system can be obtained by
standard coordinate transformation.
2.3 Formulation of Finite Element Model
Axisymmetric formulation for transient analysis can be written as:
[ ]{ } [ ]{ } { } { }e e e e e eTM K F F (11)
where[ ] 2 [ ] [ ]e T
sM N N rdS , [ ] 2 [ ] [ ][ ]e T
sK B C B rdS , { } {{ } { } { } }e T
r zu u u ,
{ }eF and { }eTF are forces due to mechanical and thermal loads respectively. In addition,
N is an interpolation function, B is the strain displacement function, C is the elasticity
matrix, is the density, and , , r zu u u are displacement components in the cylindrical
coordinate system.
By discretizing Eq. (2), the heat conduction formulation can be expressed as
[ ]{ } [ ]{ } { }T T TC T K T H (12)
where
[ ] TT p
V
C C N NdV , [ ] TT
V
K N k N dV , [ ] T TT s r
S V
H N q dS N q dV .
where k is thermal conductivity, sq is surface heat flux and rq is the reaction heat due to
resin decomposition and vaporous migration.
The reaction heat rq can be expressed as
( ) ( )r g pg pg pTq m C Q C C T Tr t
(13)
where, pgC is the specific heat of gas, T is ambient temperature and Q is the heat of
decomposition.
56
Combining Eq. (11) and (12), the sequentially coupled thermalstress equation can be
written as:
0 0 000 00 0 0
ee ee ee
T T
KMTC KT
{ }
eT
T
F FH
(14)
3. MATERIAL MODELS
3.1 Temperature Dependent Material Properties
Mechanical and thermal properties of fiber reinforced composites vary significantly
with temperature. As the carbon/epoxy laminate carries the pressure loading from the
hydrogen gas, the effect of temperature on its material properties cannot be ignored.
However, a complete set of temperature dependent properties is not available in the
literature. Assumptions and curve fittings are necessary to obtain the material property
data based on the limited experimental data that is available. Numerous studies have been
done on curve fitting of temperature dependent properties. Gibson et al. [19] shows that a
hyperbolic tan (tanh) function is capable of giving an excellent fit to experimental data
for material moduli and strength. The equation can be expressed as:
( ) tanh 2 2
U R U Rg
P P P PP T k T T C (15)
where, ( )P T is the temperature dependent material property, UP is the unrelaxed (low
temperature) value of that property, RP is the relaxed (high temperature) value of that
property, k is a constant describing the width of the distribution,T is temperature, gT is the
mechanically determined glass transition temperature and C is a constant.
57
Experimental data for carbon/epoxy composite are taken from the literature [2022].
Moduli are fitted using Eq. (15). The curve fitting parameters are listed in Table 1. The
thermal properties of carbon/epoxy are listed in Table 2 and Table 3. Properties for the
resin reaction model are listed in Table 4.
The strength of the composite is dependent on temperature and resin content. It has
been assumed that the temperature variation of the ultimate longitudinal, transverse and
shear strengths of carbon/epoxy follow the same pattern as the longitudinal, transverse
and shear moduli respectively and resin content only affects the transverse and shear
strengths. The virgin strengths used this investigation are listed in Table 5.
3.2 Composite Failure Criteria
As the composite wall of the hydrogen cylinder experiences combined mechanical
and thermal loads, a variety of failure types would occur in the process. A progressive
failure model is employed in this study to identify the failure types based on failure
criterion and predict the safety state of the cylinder. Hashin’s failure criterion [23],
accounting for four possible modes of ply failure, is used for this purpose.
1. Matrix tensile or shear cracking ( 22 33 0 )
2 2 2 222 33 12 13 23 22 33
2 2mt t ST LT
IF F
(16)
2. Matrix compressive or shear cracking ( 22 33 0 )
2 2 2 2 222 33 12 13 23 22 33
22 33 2 21 1
2 4
cT
mc c S S ST LT LT LT
FIF F F F
(17)
3. Fiber tensile fracture ( 11 0 )
58
2
2 21112 132
1ft t S
L LT
IF F
(18)
4. Fiber compressive fracture ( 11 0 )
11fc c
L
IF
(19)
where, tLF , c
LF , tTF , c
TF and SLTF are longitudinal tensile strength, longitudinal compressive
strength, transverse tensile strength, transverse compressive strength and shear strength of
unidirectional ply respectively.
Once a specific type of failure is identified in the laminate, the reduction in its load
carrying capacity is accounted for, by a reduction in its elastic moduli based on Tan's
assumption [24]: (a) When matrix tensile or shear cracking occurs, properties
22 12 23( , , )E G G are taken as 0.2 times the original values. (b) When matrix
compressive or shear cracking occurs, properties 22 12 23( , , )E G G are taken as 0.4 times
the original values. (c) When fiber tensile fracture occurs, 11E is taken as 0.07 times the
original values. (d) When fiber compressive fracture occurs, 11E is taken as 0.14 times
the original values.
3.3 Model for Hydrogen Gas
The hydrogen gas in the cylinder absorbs energy and increases the internal pressure.
In the present study, the hydrogen gas effect is modeled as a sink whose temperature is
updated at each increment based on the amount of heat flux going through the inner
cylinder surface. The internal pressure of the cylinder is computed from the state equation
of hydrogen. Experimental data for hydrogen gas is taken from the literature [25]. The
59
pressure and temperature relationship at a constant density of 23.59 kg/m3 (when the
temperature is 20°C and the pressure is 34.5 MPa) is curve fitted as shown in Figure 2.
The fitted equation is employed to compute cylinder internal pressure.
4. FINITE ELEMENT SIMULATION PROCEDURE
The cylinder dimensions used in the present study are based on the design proposed
by Mitlitsky et al. [26] and are summarized in Table 6. An axisymmetric finite element
model is built in ABAQUS as shown in Figure 3. The length of the cylindrical part is
taken as 0.3cL for analysis and the dome curve follows a geodesic path. The flame
source is modeled as a constant heat flux (75 kW/m2) applied on the area with length sL
throughout the analysis. The radiation, as well as the convection, is also considered at the
cylinder outside surface. Pressure is imposed on the inner liner surface. A symmetric
boundary condition is applied at the end of the cylinder to reduce the model to half of the
cylinder. The model uses SAX8RT element accounting for both deformation and heat
transfer. The cylinder wall consists of a inner aluminum liner and six sublaminates of
carbon/epoxy (Figure 4). Each hoop (90) and helical (±10) sublaminate consists of
many laminas.
The implementation procedure of the developed models in ABAQUS is summarized
as shown in Figure 5 and the names of interface subroutines are listed in parentheses. At
each increment, the material properties are updated (using subroutine USDFLD) based on
the information of current temperature, failure type and resin content. The mechanical
loading vector is computed from the hydrogen gas model (in the subroutine FILM). The
60
hydrogen gas model provides the sink temperature from which the internal pressure of
the cylinder is computed (from subroutine DLOAD) using the gas state equation. For
thermal loading vector, the flame source, resin decomposition, and mass flux of burning
gas contribute the heat flux collaboratively (calculated in subroutine HETVAL). The
coupled thermomechanical equations are then solved to get the global stresses and
temperature field. The lamina stresses are retrieved from global stresses and imported
into the failure model to compute failure indices. At the next increment, all submodels
(resin submodel, hydrogen gas submodel and material strength submodel) are solved
based on the temperature field and failure type from the previous increment. The
procedure iterates until the specified time is met. In the present study, this transient
analysis is carried out for 1000 seconds.
5. RESULTS AND DISCUSSION
The heat exchange rate between the hydrogen gas and aluminum liner affects the
increase in sink temperature (temperature of hydrogen gas) when the cylinder is subjected
to flame impingement. In the simulation, the heat exchange rate is represented by a film
coefficient (H). A parametric study is conducted on H ranging from 10 to 10,000
W/m2/°C. The results are shown in Figure 6. The sink temperature increases rapidly with
H at the beginning and flattens out at higher values of H. At higher H values, the sink
temperature is not sensitive to the heat exchange rate. In real situations, this value can
vary over a large range with variation of hydrogen flow rate. H is taken as 1000 W/m2/°C
for convenience throughout the analysis. Figure 7 plots the internal pressure variation
with time for different flame impingement sizes. The nondimensional L is defined as
61
L=Ls/Lc (Figure 3). It can be seen that at the beginning the internal pressure increases
very slowly and is much higher after 200 seconds. With increasing size of the flame area,
the pressure goes up. For the rest of analysis, results are reported at L = 0.1.
Figure 8 shows the temperature distributions of the liner internal surface at different
times. The temperature of flame impingement center is higher than the adjacent areas.
Figure 9 shows the temperature distributions of the composite through the thickness
direction at the flame center. The temperature of the outermost sublaminate 6 increases
to 520°C in the first 200 seconds and then continues to go up very slowly during the rest
of the time. The innermost sublaminate 1 increases slowly during the entire flame
impingement process. Figure 10 shows the residual resin content in the composite
through the thickness at the flame center. In the outermost sublaminate 6, resin is
depleted totally in the first 100 seconds and in the innermost sublaminate 1, the resin
content keeps almost constant throughout the entire process.
Stress distributions through the composite thickness at the end of the simulation time
are reported in Figures 11 and 12. An uneven stress (S11) distribution is observed in the
fiber direction for hoop sublaminates. This can result in the breakage of fibers in the
inner hoop layers. The stresses in the transverse direction (S22) and thickness direction
(S33) are plotted in Figure 12. The shear stresses are not reported as they are negligibly
small.
Failures due to fiber fracture, matrix cracking and resin depletion are presented in
Figure 13 (ac). A higher fiber fracture index is observed for the inner layer. This is
because the fibers of outer layers cannot bear much mechanical load as the resin is either
depleted or softened due to the high temperature. Matrix cracking is observed at the inner
62
half of the composite wall. However, the matrix failure index is very low at the outermost
layers, since there is not much matrix (resin) left. Hence, no significant mechanical
loading can be carried in this part. This can be observed in Figure 13(c).
6. CONCLUSIONS
A comprehensive finite element model has been developed to analyze composite
hydrogen storage cylinders subjected to high pressure and flame impingements. The
model considers the resin reaction, heat exchange between the hydrogen gas and liner,
and the progressive failure process. A sublaminate model has been developed to reduce
the computational time. A temperature dependent material model and the failure models
have been developed and implemented to accurately predict various types of failure for
the hydrogen storage cylinder. All the models are formulated in an axisymmetric
coordinate system and implemented in ABAQUS through user subroutines. Analysis of a
typical high pressure composite hydrogen cylinder under fire exposure is conducted by
using the developed model. Parametric studies are done on heat exchange rate (between
hydrogen gas and liner) and the size of flame source. Stresses, temperature profile and
failure types are reported. The developed model can be used to accommodate various
types of thermal and mechanical loadings, lamina stacking sequence, and lamina
thickness to establish safe working conditions and design limits for hydrogen storage
cylinders. In addition, this simulation process can be used for both type III and type IV
hydrogen cylinders, as both have a similar structure except for the type of liner being
used.
63
REFERENCES
[1] C. Liang, H. Chen and C. Wang, “Optimum Design of Dome Contour for Filamentwound Composite Pressure Vessels Based on a Shape Factor,” Composite Structures, Vol. 58, pp. 469482, 2002.
[2] V. V. Vasiliev, A. A. Krikanov and A. F. Razin, “New Generation of Filament
wound Composite Pressure Vessels for Commercial Applications,” Composite Structures, Vol. 62, pp. 449459, 2003.
[3] P. Y. Tabakov and E. B. Summers, “Layup Optimization of Multilayered
Anisotropic Cylinders Based on a 3D Elasticity Solution,” Computers and Structures, Vol. 84, pp. 374384, 2006.
[4] D. Chapelle and D. Perreux, “Optimal Design of a Type 3 Hydrogen Vessel: Part I
Analytic Modeling of the Cylindrical Section,” International Journal of Hydrogen Energy, Vol.31, pp. 627–638, 2006.
[5] J. Park, C. Hong and C. Kim, “Analysis of Filament Wound Composite Structures
Considering the Change of Winding Angles through the Thickness Direction,” Composite Structures, Vol. 55, pp. 6371, 2002.
[6] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load
Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247255, 2000. [7] D. L. Gray and D. J. Moser “Finite Element Analysis of a Composite Overwrapped
Pressure Vessel,” 40th AIAA/ASME/SAE/ASEE Joint Propulsion Conference and Exhibit, Fort Lauderdale, FL, AIAA 20043506, pp. 115, July 1114, 2004.
[8] I. H. Akcay and I. Kaynak, “Analysis of Multilayered Composite Cylinders under
Thermal Loading,” Journal of Reinforced Plastics and Composites, Vol. 24, pp. 11691179, 2005.
[9] O. Sayman, “Analysis of Multilayered Composite Cylinders under Hygrothermal
Loading,” Composites: Part A, Vol. 36, pp. 923933, 2005. [10] J. B. Henderson, J. A. Wiebelt and M. R. Tant, “A Model for the Thermal Response
of Polymer Composite Materials with Experimental Verification,” Journal of Composite Materials, Vol. 19, pp. 579595, 1985.
[11] J. B. Henderson and T. E. Wiecek, “A Mathematical Model to Predict the Thermal
Response of Decomposing, Expanding Polymer Composites,” Journal of Composite Materials, Vol. 21, pp. 373393, 1987.
[12] A. G. Gibson, P. N. H. Wright and YS. Wu, “The Integrity of Polymer Composites
during and after Fire,” Journal of Composite Materials, Vol. 38, pp. 12831307, 2004.
[13] K. J. Laidler, “Theories of Chemical Reactions Rates,” McGrawHill: New York,
1969. [14] J. Lua, J. O'Brien, C. T. Key, Y. Wu and B. Y. Lattimer, “A Temperature and Mass
Dependent Thermal Model for Fire Response Prediction of Marine Composites,”
64
Composites Part A: Applied Science and Manufacturing, Vol. 37, pp.10241039, 2006.
[15] P. C. Chou and J. Carleone, “Elastic Constants of Layered Media,” Journal of
Composite Materials, Vol. 6, pp. 8093, 1972. [16] C. T. Sun and S. Li, “Threedimensional Effective Elastic Constants for Thick
Laminates,” Journal of Composite Materials, Vol. 22, pp. 629639, 1988. [17] H. Chen and S. W. Tsai, “Threedimensional Effective Moduli of Symmetric
Laminates,” Journal of Composite Materials, Vol. 30, pp. 906916, 1996. [18] J. Whitcomb and J. Noh, “Concise Derivation of Formulas for 3D Sublaminate
Homogenization,” Journal of Composite Materials, Vol. 34, pp. 522535, 2000. [19] A. G. Gibson, Y.S. Wu, J. T. Evans and A. P. Mouritz, “Laminate Theory Analysis
of Composites under Load in Fire,” Journal of Composite Materials, Vol. 40, pp. 639658, 2006.
[20] K. J. Yoon and J. Kim, “Prediction of Thermal Expansion Properties of
Carbon/Epoxy Laminates for Temperature Variation,” Journal of Composite Materials, Vol. 34, pp. 90100, 2000.
[21] G. Kalogiannakis, D. V. Hemelrijck and G. V. Assche, “Measurements of Thermal
Properties of Carbon/Epoxy and Glass/Epoxy using Modulated Temperature Differential Scanning Calorimetry,” Journal of Composite Materials, Vol. 38, pp. 163175, 2004.
[22] G. Liang, A. Garg, K. Chandrashekhara, V. Flanigan and S. Kapila, “Cure
Characterization of Pultruded Soybased Composites,” Journal of Reinforced Plastics and Composites , Vol. 24, pp. 15091520, 2005.
[23] Z. Hashin, “Failure Criteria for Unidirectional Fiber Composites,” Journal of
Applied Mechanics, Vol. 47, pp. 329334, 1980. [24] S. C. Tan, “A Progressive Failure Model for Composite Laminates Containing
Openings,” Journal Composite Materials, Vol. 25, pp. 556577, 1991. [25] W. E. Deming and L. E. Shupe, “Some Physical Properties of Compressed Gases,
III. Hydrogen,” Physical Review, Vol. 40, pp. 848859, 1932. [26] F. Mitlitsky, A. H. Weisberg, and B. Myers, “Vehicular Hydrogen Storage using
Lightweight Tanks,” Proceedings of the 2000 U.S.DOE Hydrogen Program Review, NREL/CP57028890, pp. 182, 2000.
65
LIST OF TABLES
Table 1 Curve fitting parameters for transverse and shear modulus
Table 2 Thermal expansion coefficients of carbon/epoxy
Table 3 Specific heat and thermal conductivity of carbon/epoxy
Table 4 Parameters for resin reaction model
Table 5 Strength of carbon/epoxy
Table 6 Design parameters for the cylinder
66
LIST OF FIGURES
Figure 1 Schematic of hydrogen cylinder
Figure 2 Curve fitting for hydrogen gas state equation at constant density
Figure 3 Finite element model of the cylinder
Figure 4 Stacking sequence of the cylinder wall
Figure 5 Finite element implementation schemes
Figure 6 Variation of sink temperature with film coefficient
Figure 7 Internal pressure variation with time for various flame area sizes
Figure 8 Temperature distributions along the length at inner surface of the aluminum liner
Figure 9 Temperature distributions through composite thickness
Figure 10 Residual resin content through the thickness
Figure 11 Stress (S11) distribution through the thickness
Figure 12 Stress (S22, S33) distribution through the thickness
Figure 13(a) Fiber fracture index (Imt) contour around heat source
Figure 13(b) Matrix cracking index (Ift) contour around heat source
Figure 13(c) Density index (ρ/ρ0) contour around heat source
67
Table 1 Curve fitting parameters for transverse and shear modulus
Longitudinal
modulus
Transverse
modulus
Shear
modulus
PU(GPa) 133.35 9.135 4.515
PR(GPa) 111 0.1 0.045
K 0.0064 0.022 0.02
C 1 1 1
Tg (oC) 100 100 100
68
Table 2 Thermal expansion coefficients of carbon/epoxy
Temperature (oC) 1(1×106/ oC) 2(1×106/ oC)
20 1.47 29.2
40 0.97 29.5
60 0.77 33.2
80 0.81 40.0
100 1.09 50.2
120 1.61 63.6
140 2.37 80.4
350 9.03 238.0
69
Table 3 Specific heat and thermal conductivity of carbon/epoxy
Specific heat
Temperature (oC) Cp (kJ/kg/oC)
0 0.8
20 0.86
70 1.08
95 1.28
120 1.4
170 1.5
260 1.67
350 1.84
Thermal conductivity (W/m/oC)
K11 = 6.5
K22 = 0.65
K33= 0.65
70
Table 4 Parameters for resin reaction model
Properties Values
Preexponential factor, A(1/sec) 500.0
Activation energy, EA (kJ/kgmole) 6.05×104
Gas constant, R (kJ/kgmole/ oC) 8.314
Specific heat of gas, Cpg (J/kg/ oC) 2386.5
Specific heat of composite, Cp (J/kg/ oC) 1066.0
Heat of decomposition, Q (J/kg) 3.5×105
71
Table 5 Strength of carbon/epoxy
t
LF cLF t
TF cTF S
LTF Strengths
(MPa) 2463 1070 40 170 60
72
Table 6 Design parameters for the cylinder
Parameters Values
Outside diameter (m) 0.462
Liner thickness (mm) 2.54
Composite thickness (mm) 11.3
Thickness ratio (helical/hoop) 0.65
Stress ratio (helical/hoop) 0.8
Operation pressure (MPa) 34.5
Factor of safety 2.25
73
Figure 1 Schematic of hydrogen cylinder
74
0 100 200 300 400 500300
400
500
600
700
800
900
1000
Temperature (oC)
Pres
sure
(Bar
)
Fitting curveTest data
Equation: P = 1.2 T + 320
Figure 2 Curve fitting for hydrogen gas state equation at constant density
75
Figure 3 Finite element model of the cylinder
Hydrogen gas
cL
sL
Central axis of axisymmetirc model
Symmetric boundary
Flame source
76
Figure 4 Stacking sequence of the cylinder wall
oSublaminate 6 (90 ) oSublaminate 5 ( 10 )
oSublaminate 4 (90 ) oSublaminate 3 ( 10 )
oSublaminate 2 (90 ) oSublaminate1 ( 10 )
Aluminum Liner
Hoop
Helical
Hoop
Helical
Hoop
Helical
Carbon/epoxy composite
Flame source
Inner pressure
77
Figure 5 Finite element implementation schemes
78
0 2000 4000 6000 8000 1000020
40
60
80
100
120
H (W/m2/oC)
Tem
prat
ure
(o C)
Figure 6 Variation of sink temperature with film coefficient
79
0 200 400 600 800 100030
35
40
45
50
55
60
Time (Sec)
Pres
sure
(MPa
) L=1.0
L=0.1
L=0.5
Figure 7 Internal pressure variation with time for various flame area sizes
80
0 2.5 5 7.5 10 12.5 15150
20
40
60
80
100
120Te
mpe
ratu
re (o C
)
Time = 600 Sec
Time = 800 Sec
Time = 200 Sec
Time = 400 Sec
Time = 0 Sec
Time = 1000 Sec
Figure 8 Temperature distributions along the length at inner surface of the aluminum
liner
Distance from flame center (cm)
81
0 200 400 600 800 10000
100
200
300
400
500
600
700
Time (Sec)
Tem
pera
ture
(o C)
Sublaminate 4
Sublaminate 5
Sublaminate 2
Sublaminate 3
Sublaminate 1
Sublaminate 6
Figure 9 Temperature distributions through composite thickness
82
Figure 10 Residual resin content through the thickness
83
0 2 4 6 8 10 120
500
1000
1500
2000
Distance (mm)
S 11 (M
Pa)
Sublaminate 1 (Helical)
Sublaminate 2 (Hoop)
Sublaminate 4 (Hoop)
Sublaminate 3 (Helical)
Sublaminate 5 (Helical)
Sublaminate 6 (Hoop)
Figure 11 Stress (S11) distribution through the thickness
84
0 2 4 6 8 10 1230
25
20
15
10
5
0
5
Distance (mm)
S 22 S
33 (M
Pa)
S22
S33
Figure 12 Stress (S22, S33) distribution through the thickness
85
Figure 13(a) Fiber fracture index (Imt) contour around heat source
86
Figure 13(b) Matrix cracking index (Ift) contour around heat source
87
Figure 13(c) Density index (ρ/ρ0) contour around heat source
88
PAPER III:
FRACTURE ANALYSIS OF HYDROGEN STORAGE COMPOSITE
CYLINDERS WITH LINER CRACK ACCOUNTING FOR AUTOFRETTAGE
EFFECT
ABSTRACT
An understanding of fracture behavior is crucial to the safe installation and operation
of high pressure composite cylinders for hydrogen storage. This work has developed a
comprehensive finite element model to investigate axial surface flaws in cylinder liners
using the fracture mechanics and a globallocal finite element technique. Since the
autofrettage process has a strong influence on cylinder fracture behavior, it is also
considered in this analysis. The simulation process is broken down into three steps in
order to precisely extract fracture parameters and incorporate the autofrettage effect. In
the first step, the global model performs the autofrettage simulation to study the residual
stress with consideration of both material hardening and the Bauschinger effect. In the
second step, the global model uses residual stress to compute displacement for the local
model. Finally, in the third step, the local model extracts the values of stress intensity
factor (K) and Jintegral. Comparison is conducted on the fracture parameters with
various autofrettage levels and crack shapes. The vicinity of crack front is also studied by
the size and shape of the plastic zone, and the validity of stress intensity factor (K) and J
integral dominances is examined.
89
1. INTRODUCTION
High pressure composite cylinders have gained the intensive attention of the
automotive industry as hydrogen storage media for hydrogen vehicles [1]. These
cylinders are typically made of an aluminum liner wrapped with carbon/epoxy
composites. The composite wrap is designed to withstand high pressure loading (5,000
10,000Psi) of compressed hydrogen gas while maintaining a light weight through the use
of high strength, low density composite materials. The aluminum liner serves as the
hydrogen barrier layer since the material provides a perfect resistance for hydrogen
permeation [2]. However, this advantage is undermined by manufacturing defects that
lead to the development of cracks in the liner. Due to the driving force from the internal
pressure, continuous propagation of cracks will lead to serious leakage and eventual
failure of the cylinder. The fracture behavior of the aluminum liner, therefore, is a key
factor affecting the operational safety and design life expectancy of the cylinder.
Fracture analysis of composite cylinders stems from studies of various pipes and
vessels. Since surface flaws commonly occur in these products and propagate during
service, they are involved in most studies. In general, surface flaws are represented in the
analysis by semielliptical shapes. Fracture parameters such as the stress intensity factor
(K) and the Jintegral, which determine the crack criteria and cause of failure, are
computed along the front of a semielliptical crack [3,4]. Due to their geometric
complexity, only a few analytical solutions have been proposed to determine those
parameters with low computational cost [57]. Since those methods rely on simplified
assumptions about material models and the stress field near the crack tip, they are
suitable for a simple geometry and linear analysis.
90
The finite element (FE) method provides a more general and flexible tool for
evaluation of both stress intensity factor (K) and Jintegral, and results have been widely
reported in the literature. Rice and Levy [8] introduced a linespring element model to
compute K, and that work was expanded by Lee and Parks [9] to evaluation of Jintegral
and T stress. Raju et al. [10] computed K for internal and external surface cracks in
cylindrical vessels using a 3D continuum element. Kim et al. [11] analyzed internal axial
surface cracks in cylinders considering various geometric ratios and material plasticity.
Diamantoudis and Labeas [12] modeled the cracks at various locations on a pressure
vessel using a globallocal FE technique. Guerrero et al. [13] improved a pressure vessel
design based on a detailed FE fracture analysis. Su et al. [1416] performed fracture
analysis on a series of compressed natural gas cylinders. Based on previous studies, most
research has addressed to metallic cylinders, and few studies have focused on metallic
liners with a composite wrap in the hoop direction. Still less work has studied the full
compositewrapped cylinder with consideration of the autofrettage effect.
Autofrettage is a metal fabrication technique, commonly used in increasing durability
of highpressure cylinders, cannon barrels and diesel engines. In this technique, the
cylindrical product is subjected to enormous pressure, causing internal portions of the
part to yield and resulting in internal compressive residual stresses to enhance product
fracture performance. Since autofrettage has strong influence on cylinder fracture
behavior, this paper investigates liner cracks of high pressure composite cylinders for
hydrogen storage considering autofrettage effect using fracture mechanics and a global
local FE technique. The globallocal FE model has been developed in a commercial FE
code, ABAQUS. The autofrettage effect is studied in the global model. The local model,
91
which is driven by the results of the global model, analyzes the crack in detail to ensure
accurate computation of fracture parameters. Results for both K and the Jintegral are
reported for four autofrettage levels along the crack front. The effect of crack size is also
examined using cracks with various depth/thickness and depth/width ratios. In addition,
since the stress field in the vicinity of the crack tip determines the validity of fracture
parameter characterization, which is crucial for design parameter selection, the plastic
zone around the crack front is studied.
2. METHODOLOGY
A schematic of a hydrogen composite cylinder with an inner surface flaw is shown in
Figure 1. The inner liner is made of aluminum alloy that serves as a hydrogen gas
permeation barrier. Filamentwound carbon/epoxy composite laminates wrap the liner in
both the hoop and the helical directions. These laminates provide the desired pressure
load bearing capacity. Due to the inner hydrogen pressure, cracks develop as a result of
manufacturing defects and propagate in the liner wall during service. In order to restrain
crack propagation, the autofrettage process is conducted before the cylinder enters service
by introducing proper compressive stresses in the liner [17]. Stress intensity factor (K)
and the Jintegral provide a means to study the fracture performance of the cylinder
according to the various deformation states.
2.1 The Autofrettage Effect on Hydrogen Storage Composite Cylinders
The fracture resistance of composite hydrogen cylinders can be improved by the
autofrettage process, in which the cylinder is pressurized to a specified proof pressure to
produce a desired compressive stress level in the liner. Figure 2 illustrates the process
92
with stressstrain and load versus time curves. The autofrettage process is conducted in
the first cycle pressure loading (0→2→4) as shown in Figure 2(b). Afterwards, the
pressure will cyclically remain between zero and operating pressure ( 4 ↔ 4 ) in service.
During autofrettage (0→2), the composite wrap responds linearly in an elastic state,
as represented by the dotted line from 0 to A in Figure 2(a). At the same time, the liner
undergoes elastoplastic deformation represented by the solid curve (0→1→2). Large
plastic deformation is introduced in the liner when the cylinder is overstressed to the
proof pressure level. In the unloading process (2→4), the cylinder pressure returns to 0.
The composite wrap goes from A to C, where it remains in tension. It compresses the
liner linearly from point 2 to point 3 and plastically to point 4. At this point, the balance
between the composite wrap and the liner is established, and the compressive stress c is
introduced into the liner. During service ( 4 ↔ 4 ), the aluminum liner operates in
( 4 ↔ 4 ), and the composite wrap remains in (C↔B). The fracture analysis conducted
here focuses on the service stage.
The selection of a proof pressure is crucial for the success of the autofrettage process.
The following factors are considered in the process: (a) composite wrap strength, (b) liner
material yielding strength, (c) Bauschinger effect, and (d) liner buckling. A maximum
proof pressure selected should be smaller than the maximum pressure sustainable by the
composite wrap, with a safety margin in case of damage to the composite. There is
another tradeoff for the selection of yielding strength of liner materials. The hysteresis
loop is to be formed as the yielding strength is too low while not much compressive stress
can be introduced if it is too high. In addition, the compressive yielding strength c is
affected by the Bauschinger effect which implies extremely high proof pressure may not
93
introduce high compressive stress in the liner. Furthermore, the compressive pressure
introduced must not exceed the critical buckling stress of the liner wall, which can be
expressed as [18]:
23(1 )crit
E tRv
(1)
where E is Young’s modulus, v is Poisson’s ratio, t is the wall thickness of the liner, and
R is the cylinder radius.
2.2 Stress Intensity Factor (K) Evaluation
Since very few practical problems have closedform stress intensity factor (K)
solutions, numerical methods are widely used as an alternative for problems with
complex geometric configurations and loadings. The approaches implemented in
numerical evaluation generally fall into two categories: point matching and energy
methods [19]. Point matching method derives from the formula of stress and
displacement fields near the crack tip, but it requires a high degree of mesh refinement
for reasonable accuracy. Earlier energy methods, such as J contour integration, elemental
crack advance, and virtual crack extension, compute K based on the energy release rate in
the body; however, separation of mixedmode K components is difficult with these
methods.
An interaction integral method is used in ABAQUS to extract the individual stress
intensity factor (K) for a crack from the domain integral procedure [2021]. This method
is more accurate and efficient than earlier energy methods, and it is applicable to both
isotropic and anisotropic linear materials under monotonic loading. The expression of K
can be written as:
94
int4K B J
(2)
where K
is the K vector and intJ
is the interaction integral vector, both with three
components according to three modes, and B is a prelogarithmic energy factor matrix.
For homogeneous, isotropic materials, B is given by:
2
2
8 (1 ) / 0 00 8 (1 ) / 00 0 4 /
EB E
G
(3)
where E is Young’s modulus, v is Poisson’s ratio, and G is the shear modulus.
The interaction integral vector intJ
is evaluated by the domain integral procedure and
can be expressed as:
int limJ n M q d
(4)
with M given by:
: aux auxaux
u uM Ix x
(5)
where is equal to I, II, and III according to the three modes of fracture mechanics,
is the contour that encloses the crack tip, n is the outward normal of , q is the crack
extension direction, u is the displacement vector, x is the coordinate vector, I is the
identity matrix, and , aux and aux
are stress, auxiliary stress, and strain respectively.
2.3 JIntegral Evaluation
The energy domain integral method is formulated in [22] to provide a general
framework for numerical analysis of the Jintegral. This method has been adopted by
ABAQUS for its easier numerical implementation and higher accuracy with coarser mesh
compared with earlier energy methods. In the domain integral technique, a closed contour
95
( C C C ) is constructed around the crack as illustrated in Figure 3. The inner
contour is vanishingly small, while the outer contour C is finite. Using the divergence
theorem, the 2D quasistatic contour integral is converted to domain integral on closed
area A , which is defined by:
A C C
uJ H q d t q dx x
(6)
with tensor H given by:
uH WIx
(7)
where t
is the surface traction force, q is equal to q on and vanishes on C , and W is
the strain energy. For elastoplastic material, plastic dissipation is also included in W ,
which implies that the Jintegral calculation of this condition is applicable only for
monotonic loading. The 3D domain integral can be obtained by expanding a 2D contour
along crack front S for a virtual distance dS to form an integral on volumeV .
The ABAQUS software defines the domain in terms of rings of elements surrounding
the crack tip [21]. The first contour consists of those elements directly connected to
cracktip nodes. The second contour includes the elements in the first contour and the
next ring of elements that share nodes with the elements in the first contour. Each
subsequent contour is defined by adding the next ring of elements that share nodes with
the elements in the previous contour.
2.4 Material Models
Several material models are used in the simulation to describe the behavior of the
cylinder wall. The composite wrap is formulated by doubly curved laminated shell theory
with an orthotropic material constitutive model given by:
96
1 12 1 13 111 11
22 12 1 2 23 2 22
33 3313 1 23 2 3
12 1212
13 1313
23 2323
1/ / / 0 0 0/ 1/ / 0 0 0/ / 1/ 0 0 0
0 0 0 1/ 0 00 0 0 0 1/ 00 0 0 0 0 1/
E E EE E EE E E
GG
G
(8)
where iE is Young’s moduli, ijG is the shear moduli, and ij is Poisson’s ratios.
To simulate the autofrettage process, an elastoplastic material model is used to
capture deformation of the aluminum liner in the global model. The nonlinear
isotropic/kinematic hardening law is employed to account for the Bauschinger effect. The
yield surface is governed by the Mises flow rule:
0yf (9)
with equivalent Mises stress given by:
3 :2
dev devf S S (10)
where is the back stress, dev is the back stress deviator, and S is the stress deviator.
The hardening law is given by:
1 pl pl
y
C
(11)
where is the back stress rate, pl is the equivalent plastic strain rate, C is the kinematic
modulus, and is the slip rate. C and are calibrated by material test data.
In the submodel, different elastic models are implemented for the aluminum liner
according to computational requirement of fracture parameters. To extract K along the
crack front, linear elastic material model is required by the interaction integral method.
Instead of using an elastoplastic model, RambergOsgood (RO) nonlinear elastic model
is used in Jintegral evaluation, thus eliminating the loading effect on the accuracy of
97
domain integration. The onedimension expression of the RO model can be expressed
as:
0 0 0
n
(12)
where is a dimensionless constant and n is the strain hardening exponent. The model
is directly related to the description of the singularity field around the crack tip and it is
widely used for curvefitting the stressstrain data. The 3D format, used in the simulation,
can be expanded from Eq.(12) as:
1
0
31 1 22
nqE S pI S
(13)
where E is Young’s modulus, is Poisson’s ratio, p is the equivalent hydrostatic stress,
q is the vonMises equivalent stress, and S is the stress deviator.
Distinction between the K dominance and Jintegral dominance is characterized by
the size of the plastic zone in the vicinity of the crack tip. The radius of a critical plastic
zone is given by:
216
ICp
y
Kr
(14)
where ICK is the mode I fracture toughness and y is the yielding strength. The domain
of the plastic zone is obtained by identifying the region where the asymptotic stress ahead
of the crack tip equals the yielding stress.
98
3. FINITE ELEMENT SIMULATION
The semielliptical crack is required to be modeled in substantial detail to obtain
precise values of fracture parameters. If the crack were modeled together with the whole
cylinder, the resulting element size would be too small and the model would be too large.
Along with the complexity of wall structure and material nonlinearity, it would demand
tremendous computational cost. This restriction is resolved by a globallocal FE analysis
strategy. The global model with coarse mesh is used to obtain the displacement solution
of the liner crack region. The local model of the region surrounding the crack is created
with a very fine mesh. The boundary conditions of the local model are driven by the
solution of global analysis.
The dimensions considered in the present analysis are based on a design typical of
those described in literature [2]. The outer radius of the cylinder outR is 0.229 m and the
inner radius inR is 0.217 m (Figure 1). The carbon/epoxy wrap consists of helical and
hoop laminates resulting in a total composite shell thickness ( ct ) of 9 mm, and the
thickness of the liner ( at ) is 2.54 mm. The material properties are summarized in Tables
1 and 2 [2, 23]. Study cases with various flaw sizes and proof pressures are summarized
in Table 3.
3.1 Global Model
For symmetry, one eighth of the cylinder is modeled, and symmetric boundary
conditions are imposed on the cut sides. The laminated composite wrap is modeled using
a doubly curved 8node shell element and the liner by an 8node solid brick element.
Reduced integration is used to improve both computational efficiency and bending
analysis accuracy. Figure 4 shows a schematic of the mesh for the whole cylinder model.
99
A finer mesh is used in the region, to which the local model will be applied. The wall is
constructed by tying the shell element to the brick element surface with an offset of a half
shell thickness. The layup of composite wrap ( 0 03[ 10 / 90 ] ) consists of six helical plies
alternated with three hoop plies (in Figure 4). The thickness of each helical ply is 0.55
mm and each hoop ply is 1.9 mm in order to match the design stress ratio 0.8 (stress in
the helical layer/stress in the hoop layer). The material direction of the aluminum liner is
1 in the hoop and 2 in the axial direction. Pressure loading is applied on the entire inner
surface of the liner.
3.2 Local Model
To evaluate the fracture parameters for the axial crack, a local FE model is created for
a small portion of the liner wall containing a crack (Figure 5). The size of the region is
approximately that of one element in the global model (marked in Figure 4). The
geometry of the region is the same as the corresponding portion in the global model. In
consideration of the crack symmetry, only half the crack is modeled. Quadratic
continuum elements with 20 nodes (C3D20R in ABAQUS) are employed for better
accuracy and better representation of the crack front curvature. The mesh density is
significantly higher than that for the global model, and the crack tip is surrounded by
many layers of elements. Singular continuum elements with a collapsed face are used to
model the crack tip. For computation of K, 1/ r singularity is created using quarter
point nodes, where r is the distance to the crack tip. When the Jintegral is evaluated, the
nodes at crack tip are duplicated to create the combined1/ r and1/ r singularity for
powerlaw hardening.
100
Figure 5 shows the local FE model of the region containing a crack. The bottom face
and the area below the crack front on the front face are applied with pressure loading.
Boundary conditions of the top, back, and right faces are determined by displacement
results of the global analysis. Symmetric constraints are imposed on the left face and the
area above the crack front on the front face. The transfer of global analysis results to local
analysis is achieved using the submodeling procedure of ABAQUS software.
3.3 Simulation Procedure
The implementation scheme of the simulation procedure is illustrated in Figure 6. The
entire simulation is performed in three steps. The data swap between steps is assisted by
ABAQUS subroutines and the submodel technique. The procedure is executed
automatically by the control of Matlab software.
Step 1: The autofrettage process is simulated in the global model by applying cyclic
pressure loading. A stress state (marked as ‘ ’ in Figure 2) is selected and will be
exported to the second step analysis as initial stress. Since the domain integral method in
ABAQUS does not consider the initial stress, the stress in the liner is chosen to be close
to zero in the selected stress state. The stress state selected for the model is recorded to a
file using the ABAQUS user subroutine UVARM.
Step 2: The displacement field needed for the submodel is computed from the global
model with a monotonic pressure loading applied from zero to operating pressures. The
autofrettage effect is introduced by applying the initial stresses in the model. From the
file created in Step 1, the initial stresses are read in using the ABAQUS user subroutine
SIGINI.
101
Step 3: The fracture parameters are extracted from the local model. The model is
driven by the boundary displacement computed from Step 2. Monotonic pressure loading
identical to that in Step 2, is applied on the crack open face. Various material models are
implemented with a linear elastic model for K computation and an RO model for J
integral evaluation.
4. RESULTS AND DISCUSSION
4.1 Autofrettage Process Simulation
The farfield vonMises stress distribution of the liner with four autofrettage levels is
shown in Figure 7. The stresses are plotted as a function of pressure loading increment.
The pressure load increases linearly to proof pressure in the first ten increments (Interval
1), decreases to 0 in the next 10 increments (Interval 2), and rises back to operating
pressure in the last 10 increments (Interval 3). The yielding occurs during Interval 1, and
a higher stress level is obtained by a higher proof pressure due to material hardening.
When pressure returns to 0 at 20th increment, residual stresses are introduced by
compression of the composite wrap. Higher residual stresses occur at higher proof
pressure. At the 30th increment, when it rises back to operating pressure, lower stresses
remain in higher proof pressure cases.
Figure 8 illustrates cyclic farfield stressstrain curves for the liner at four autofrettage
levels according to the loading sequence described in Figure 7. The stress/strain aligns in
the hoop direction which is perpendicular to the crack face. The deformation routes of
four autofrettage levels are listed in the lower right corner of the figure. It can be seen
that higher compressive stress is introduced when higher proof pressure is applied, and
102
the opposite is taken for the tensile stresses. The variation of the introduced compressive
stresses is proportional to proof pressure with the exception to the case of f oP =2.0 P . The
reason is that the first three cases do not reach the compressive yielding strength and
return linearly, and the last case yields at point 5 . Also, the Bauschinger effect can be
observed at point 5 , where the yielding stress is less than that at point1. Furthermore, the
four cases satisfy all constrains specified in section 2.1 and the selected stress fields are
exported for the subsequent step analysis.
4.2 Stress Intensity Factor (K) and Jintegral
In the present section, results along the crack front are normalized to θ as shown in
the inset in Figure 9. Stress intensity factor (K) and the Jintegral along the crack front
are reported in Figures 9 and 10 respectively with four selected autofrettage levels. The
values of both K and the Jintegral at a higher θ are much larger than those at a lower θ .
This implies that the crack grows faster in the center so that the elliptic shape tends to be
stretched closer to a circular shape. It can also be observed that the autofrettage process
dramatically reduces the values of both K and the Jintegral.
Figures 11 and 12 plot K and the Jintegral against the internal pressure loading. The
dotted horizontal lines mark the critical values of parameters (or fracture toughness)
cK and cJ . At the beginning, values of fracture parameters are equal to zero, indicating the
crack is compressed to closure status by the composite wrap. With the internal pressure
increasing enough to overcome the compressive stress, the crack changes to the opening
status. Value of stress intensity factor increases with loading linearly, while that of J
integral increases nonlinearly. Furthermore, the crack for case f oP =1.0 P may stay in
unstable growth condition since both the Jintegral and K are above critical values.
103
Figures 13 to 16 show K and the Jintegral along the crack front with various
geometric ratios when the proof pressure is equal to 1.5 times the operating pressure.
Figures 13 and 14 show the results of cracks with same shape (depth/width ratio) but
different sizes (depth/thickness ratio). It can be seen that the crack size significantly
affects fracture performance and fracture parameters of a larger crack have much higher
values. Figures 15 and 16 show the results of cracks with the same size and different
shapes. When the crack shape becomes closer to a circle (higher depth/width ratio), the
curve of fracture parameters becomes flatter. Crack growth speed along crack front is
almost same when a/c is equal to 0.75. However, when a/c is equal to 0.25, the center part
of the crack grows much faster than two sides.
4.3 Stress Field Characterization on the Crack Tip Vicinity
Figure 17 shows the stress distribution around the crack tip of a typical loading
condition. The stress is relaxed in the area under the crack tip near the free crack surface,
while it is concentrated in the front of crack tip with an oblique angle where the plastic
zone is formed. In Figure 18, three locations along the crack front curve, identified as A,
B, and C, are selected to illustrate plastic zone shape and stress distribution. A plane
strain like plastic zone is developed at A , takes transition around the B and turns into the
shape of a typical plain stress plastic zone at C.
Figure 19 shows the size of the plastic zone with four autofrettage levels at A and C.
The critical plastic zone size is characterized by the radius pcr computed from Eq.(14) and
marked by dotted circles. It can be seen that large scale yielding occurs when f 0P =1.0 P .
The plastic zone grows out of the 2 pcr region, indicating fracture failure may occur by
unstable crack growth. When f 0P =1.25 P , the size of the plastic zone is large, compared
104
with dimensions of the crack length and the remaining ligament, which implies a
contained yielding condition. When f 0P =1.5 P , the plastic zone size is small enough for
the Jdominated stress field to be developed around the crack tip and the crack tip
condition can be characterized by the Jintegral. Based on the ASTM standard, the case
of f 0P =2.0 P can be safely characterized by one K parameter since the size of its plastic
zone is at least fifteen times smaller than the other dimensions.
5. CONCLUSIONS
A comprehensive finite element model has been developed to predict the fracture
behavior of high pressure composite cylinders for hydrogen storage. The simulation of
the autofrettage process is carried out in the global model. Plastic hardening and
Bauschinger effect are observed in the results. Both stress intensity factor (K) and the J
integral are computed along the crack front in the local model with consideration of
autofrettage influence and crack size effect. Results show that the autofrettage process
significantly improves the cylinder fracture performance, and the smaller crack size
reduces the values of the fracture parameters dramatically. Shape and size of the plastic
zone around the crack tip are examined. Fracture behavior is evaluated by observation of
the plastic zone, and the corresponding parameter characterization is analyzed. The
developed model and the proposed methodology can be used for design guidance to
improve cylinder fracture performance with consideration of autofrettage process, and
developing a fracture parameter database for fatigue life prediction.
105
REFERENCES
[1] D. Chapelle and D. Perreux, “Optimal Design of a Type 3 Hydrogen Vessel: Part IAnalytic Modeling of the Cylindrical Section,” International Journal of Hydrogen Energy, Vol.31, pp. 627–638, 2006.
[2] F. Mitlitsky, A. H. Weisberg and B. Myers, “Vehicular Hydrogen Storage using Lightweight Tanks, ” Proceedings of the 2000 U.S.DOE Hydrogen Program Review, NREL/CP57028890, 2000.
[3] H. Kobayashi, S. Sakai, M. Asano, K. Miyazaki, T. Nagasaki and Y. Takahashi, “Development of a Flaw Evaluation Handbook of the High Pressure Institute of Japan,” International Journal of Pressure Vessels and Piping, Vol.77, pp.929936, 2000.
[4] A. R. Shahani and S. E. Habibi, “Stress Intensity Factors in a Hollow Cylinder Containing a Circumferential Semielliptical Crack Subjected to Combined Loading,” International Journal of Fatigue, Vol. 29, pp.128140, 2007.
[5] J. H. Underwood, “Stress Intensity Factor for Internally Pressurized Thick Walled Cylinders,” ASTM STP, Vol. 513, pp. 59–70, 1972.
[6] I. S. Raju and J. C. Newman, “An Empirical Stress Intensity Factor Equation for the Surface Crack,” Engineering Fracture Mechanics, Vol.15, pp. 185192, 1981.
[7] T. Fett, “Estimation of Stress Intensity Factors for Semielliptical Surface Cracks,” Engineering Fracture Mechanics, Vol. 66, pp.349356, 2000.
[8] J. R. Rice and N. Levy, “The Partthrough Surface Crack in an Elastic Plate,” Journal of Applied Mechanics, ASME, Vol. 39, pp.185194, 1972.
[9] H. Lee and M. Parks, “Enhanced Elasticplastic Linespring Finite Element,” International Journal of Solids and Structures, Vol. 32, pp. 23932418, 1995.
[10] I. S. Raju and J. C. Newman, “Stressintensity Factor for Internal and External Surface Cracks in Cylindrical Vessels,” International Journal of Pressure Vessel Technology, Vol.104, pp.293298, 1982.
106
[11] YJ Kim, JS Kim, YJ Park and YJ Kim, “Elastic–plastic Fracture Mechanics Method for Finite Internal Axial Surface Cracks in Cylinders,” Engineering Fracture Mechanics, Vol.71, pp.925944, 2004.
[12] A. Th. Diamantoudis and G. N. Labeas, “Stress Intensity Factors of Semielliptical Surface Cracks in Pressure Vessels by Globallocal Finite Element Methodology,” Engineering Fracture Mechanics, Vol. 72, pp.12991312, 2005.
[13] M. A. Guerrero, C. Betegon and J. Belzunce, “Fracture Analysis of a Pressure Vessel Made of High Strength Steel (HSS),” Engineering Failure Analysis, Vol.15, pp.208219, 2008.
[14] B. Su and G. S. Bhuyan, “The Fracture Behavior of the Aluminum Lined Hoopwrapped Cylinders with Internal Axial Cracks,” International Journal of Pressure Vessels and Piping, Vol. 76, pp.251257, 1999.
[15] B. Su, Ch. Li and G. S. Bhuyan, “Comparison between Fractures Parameters of an Allaluminum Cylinder with Cracks under Different Deformation Conditions,” International Journal of Pressure Vessels and Piping, Vol.77, pp. 179184, 2000.
[16] A. R. Shahani and M. M. Kheirikhah, “Stress Intensity Factor Calculation of Steellined Hoopwrapped Cylinders with Internal Semielliptical Circumferential Crack,” Engineering Fracture Mechanics, Vol.74, pp. 20042013, 2007.
[17] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247255, 2000.
[18] G. W. Hunt, G. J. Lord and M. A. Peletier, “Cylindrical Shell Buckling: A Characterization of Localization and Periodicity,” Discrete and Continuous Dynamical Systems – Series B, Vol. 3, pp. 505518, 2003.
[19] T. L. Anderson, Fracture mechanics: Fundamentals and Applications. Boca Raton, Florida: CRC Press, 1995.
[20] C. F. Shih and R. J. Asaro, “Elastoplastic Analysis of Cracks on Bimaterial Interfaces: Part I–Small Scale Yielding,” Journal of Applied Mechanics, ASME, Vol. 55, pp. 299–316, 1988.
[21] ABAQUS version 6.7. Pawtucket, RI: Hibbitt, Karlsson & Sorensen Inc, 2007.
107
[22] B. Moran and C. F. Shih, “A General Treatment of Crack Tip, Contour Integrals,” International Journal of Fracture, Vol. 35, pp.295–310, 1987.
[23] J. B. Jordon, M. F. Horstemeyer, K. Solanki and Y. Xue, “Damage and Stress State Influence on the Bauschinger Effect in Aluminum Alloys,” Mechanics of Materials Vol. 39, pp. 920–931 2007.
108
LIST OF TABLES
Table 1 Mechanical properties of carbon/epoxy composite
Table 2 Mechanical properties of Aluminum Alloy 7075T651
Table 3 Summary of study cases
109
LIST OF FIGURES
Figure 1 Schematic of hydrogen composite cylinder
Figure 2 Diagram of autofrettage process
Figure 3 Schematic of domain integral evaluation
Figure 4 Global finite element model
Figure 5 Local finite element model
Figure 6 Implementation scheme
Figure 7 vonMises stress distribution in liner
Figure 8 Cyclic stressstrain curves for various autofrettage levels
Figure 9 Stress intensity factor (K) along crack front for various autofrettage levels
Figure 10 Jintegral along crack front for various autofrettage levels
Figure 11 Stress intensity factor (K) against pressure loading for various autofrettage
levels
Figure 12 Jintegral against pressure loading for various autofrettage levels
Figure 13 Stress intensity factor (K) along crack front with various geometric ratios
Figure 14 Jintegral along crack front with various geometric ratios
Figure 15 Stress distribution of the crack front vicinity
Figure 16 Transition of plastic zone shapes along crack front
Figure 17 Plastic zone shapes for various autofrettage levels
110
Table 1 Mechanical properties of carbon/epoxy composite
Properties Values
E1 (GPa) 156.5
E2 , E3(GPa) 7.23
G12 ,G13(GPa) 4.12
G23(GPa) 3.35
12 , 13 0.337
23 0.4
Fiber strength (MPa) 5100
111
Table 2 Mechanical properties of Aluminum Alloy 7075T651
Properties Values
E (GPa) 71.7
12 0.33
y (MPa) 520
c (MPa) 430
n 25
0.3
C (GPa) 7.0
40
112
113
Figure 1 Schematic of hydrogen composite cylinder
114
Figure 2 Diagram of autofrettage process
u
op
CompositeultimatestressLiner yieldingstressLiner compressive yieldingstressLiner compressive stress
Liner tensilestressCompositeultimatestrainOperatingstrain
Applied pressure
comu
yyc
c
t
p
0
p Proof pressureOperatingpressure
t
2
4
4
0
12
4
comu
y
c
op
yc
ut
Proof pressure state
Operating pressure stateComposite
D
4
A
B
C
3(a)
(b)4
115
Figure 3 Schematic of domain integral evaluation
1x
2x
3x
crack front
crack front
m
q
m
C
S
dS
A
V
+C
C
outward normalon theclosed contourvirtualcrack extensiondirection vector
m
q
116
Figure 4 Global finite element model
117
Figure 5 Local finite element model
Front face
Left face
Bottom face
Top faceBack face
Right face
Crack front
118
Figure 6 Implementation scheme
119
Figure 7 vonMises stress distribution in liner
0 5 10 15 20 25 300
100
200
300
400
500
600
700
Step Inc
von
Mis
es(M
Pa)
f oP =1.25 Pf oP =1.50 Pf oP =2.00 P
f oP =1.00 P
120
Figure 8 Cyclic stressstrain curves for various autofrettage levels
121
Figure 9 Stress intensity factor (K) along crack front for various autofrettage levels
0 10 20 30 40 50 60 70 80 905
10
15
20
25
30
35
40
(Degree)
K (M
Pa
m)
a
a/c=1/4a/t 1/ 2
θ aat2c
f 0P =P
f 0P =1.25 P
f 0P =1.5 P
f 0P =2.0 P
122
Figure 10 Jintegral along crack front for various autofrettage levels
0 10 20 30 40 50 60 70 80 900
5
10
15
20
(Degree)
J (k
Pa
m)
a
a/c=1/4a/t 1/ 2
f 0P =P
f 0P =1.25 P
f 0P =1.5 P
f 0P =2.0 P
123
Figure 11 Stress intensity factor (K) against pressure loading for various autofrettage
levels
0 5 10 15 20 25 30 3540
30
20
10
0
10
20
30
40
Loading pressure (MPa)
K (M
Pa
m)
a
a/c=1/4a/t 1/ 2 f 0P =P
f 0P =1.5 P
f 0P =2.0 P
f 0P =1.25 P
cK
cK
124
Figure 12 Jintegral against pressure loading for various autofrettage levels
0 5 10 15 20 25 30 350
5
10
15
20
Loading pressure (MPa)
J (k
Pa
m)
f 0P =P
f 0P =1.5 P
f 0P =2.0 P
a
a/c=1/4a/t 1/ 2
f 0P =1.25 P
CJ
125
Figure 13 Stress intensity factor (K) along crack front with various geometric ratios
0 10 20 30 40 50 60 70 80 906
8
10
12
14
16
18
20
(Degree)
K (M
Pa
m)
f 0
a/c=1/4P =1.5 P
aa/t =0.25
aa/t =0.50
aa/t =0.75
126
Figure 14 Jintegral along crack front with various geometric ratios
0 10 20 30 40 50 60 70 80 900
1
2
3
4
5
(Degree)
J (k
Pa
m)
f 0
a/c=1/4P =1.5 P
aa/t =0.25
aa/t =0.50
aa/t =0.75
127
Figure 15 Stress distribution of the crack front vicinity
128
Figure 16 Transition of plastic zone shapes along crack front
A B C
Plastic zone
129
Figure 17 Plastic zone shapes for various autofrettage levels
(b) At location C 1 0.5 0 0.5 1
0
0.5
1
1.5
Length (mm)
Leng
th (m
m)
Crack face pcr
pc2r
f oP =1.0×P
f oP =1.25×P
f oP =1.5×Pf oP =2.0×P
(a) At location A
1 0.5 0 0.5 10
0.5
1
1.5
Length (mm)
Leng
th (m
m)
Crack facepcr
pc2r
f oP =1.0×P
f oP =1.25×P
f oP =1.5×P
f oP =2.0×P
130
BIBLIOGRAPHY
[1] Züttel, “Materials for Hydrogen Storage,” Materials Today, Vol.6, pp.2433, 2003. [2] N. Takeichi, H. Senoh and T. Yokota, “‘Hybrid Hydrogen Storage Vessel’, a Novel
Highpressure Hydrogen Storage Vessel Combined with Hydrogen Storage Material,” International Journal of Hydrogen Energy, Vol.28, pp.11211129, 2003.
[3] E. David, “An Overview of Advanced Materials for Hydrogen Storage,” Journal of
Materials Processing Technology, Vol.162163, pp.169177, 2005. [4] J. M. Lifshitz and H. Dayan, “Filamentwound Pressure Vessel with Thick Metal
Liner,” Composite Structures, Vol.32, pp.313323, 1995. [5] D. V. Rosato and C. S. Grove “Filament Winding, Its Development, Manufacture,
Applications and Design,” New York: Interscience, 1964. [6] A. M. Shibley, “Filament winding, Handbook of Fiberglass and Advanced Plastic
Materials,” New York: Van Nostrand Reinhold, 1969. [7] S. T. Peters, W. D. Humphrey and R. F. Foral, “Filament Winding Composite
Structure Fabrication,” Advancement of Material and Process Engineering, SAMPE International Business Office, 1991.
[8] S. G. Lekhnitskii, “Theory of Elasticity of an Anisotropic Body,” Moscow: Mir
Publishers, 1981. [9] J. Mistry, A. G. Gibson and YS. Wu, “Failure of Composite Cylinders under
Combined External Pressure and Axial Loading,” Composite Structures, Vol.22, pp.193200, 1992.
[10] P. D. Soden, R. Kitching, P. C. Tse, M. J. Hinton and Y. Tsavalas, “Influence of
Winding Angle on the Strength and Deformation of Filamentwound Composite Tubes Subjected to Uniaxial and Biaxial Loads,” Composites Science and Technology, Vol.46, pp.363–378, 1993.
[11] M. F. S. AlKhalil, P. D. Soden, R. Kitching and M. J. Hinton, “The Effects of
Radial Stresses on the Strength of Thinwalled Filament Wound GRP Composite Pressure Cylinders,” International Journal of Mechanical Science,Vol.38, pp.97120, 1996.
[12] P. M. Wild and G. W. Vickers, “Analysis of Filamentwound Cylindrical Sheels
under Combined Centrifugal, Pressure and Axial Loading,” Composite Part A, Vol.28, pp.4755, 1997.
131
[13] L. Parnas and N. Katırc, “Design of Fiberreinforced Composite Pressure Vessels under Various Loading Conditions,” Composite Structure, Vol.58, pp.8395, 2002.
[14] H. Akcay and I. Kaynak, “Analysis of Multilayered Composite Cylinders under
Thermal Loading,” Journal of Reinforced Plastics and Composites, Vol. 24, pp.11691179, 2005.
[15] O. Sayman, “Analysis of Multilayered Composite Cylinders under Hydrothermal
Loading,” Composites: Part A, Vol.36, pp.923933, 2005. [16] P. Y. Tabakov, “Design of Laminated Cylinders using Genetic Algorithm,” Journal
of Applied Computer Science, Vol.8, pp.729, 2000. [17] P. Y. Tabakov and E. B. Summers, ”Layup Optimization of Multilayered
Anisotropic Cylinders based on a 3D Elasticity Solution,” Computers and Structures, Vol.84, pp.374384, 2006.
[18] D. Chapelle and D. Perreux, “Optimal Design of a Type 3 Hydrogen Vessel: Part I
Analytic Modeling of the Cylindrical Section,” International Journal of Hydrogen Energy, Vol.31, pp.627 638, 2006.
[19] S. V. Hoa, C. H. Yu and T. S. Sankar, “Analysis of Filament Wound Vessel Using
Finite Elements,” Composite Structures, Vol. 3, pp.118, 1985. [20] J. Park, C. Hong, CG. Kim and CU. Kim, “Analysis of Filament Wound
Composite Structures considering the Change of Winding Angles through the Thickness Direction,” Composite Structures, Vol. 55, pp.6371, 2002.
[21] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load
Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247255, 2000. [22] H. T. Walter, P. S. Griffin and A. C. Jackson, “Design and Manufacture of a
Composite Overwrapped Pressurant Tank Assembly,” 38th AIAA/ASME/SAE/ASEE Joint Propulsion Conference & Exhibit, Indianapolis, Indiana, AIAA 20024349, pp.112, 2002.
[23] D. L. Gray and D. J. Moser, “Finite Element Analysis of a Composite Overwrapped
Pressure Vessel,” 40th AIAA/ASME/SAE/ASEE Joint Propulsion Conference and Exhibit, Fort Lauderdale, Florida, AIAA 20043506, pp.115, 2004.
[24] U. Kim, J. Kang, C. Hong and C. G. Kim, “Optimal Design of Filament Wound
Structures under Internal Pressure based on the Semigeodesic Path Algorithm,” Composite Structures, Vol. 67, pp.443452, 2005.
132
[25] Y. D. Doh and C. S. Hong, “Progressive Failure Analysis for Filament Wound Pressure Vessel,” Journal of Reinforced Plastics and Composites, Vol.14, pp.12781306, 1995.
[26] C. Chamis, P. K. Gotsis and L. Minnetyan, “Progressive Fracture and Damage
Tolerance of Composite Pressure Vessels,” Proceedings of The International Composites Expo, Session 5C, pp.18, 1997.
[27] L. Minnetyan, P. K. Gotsis and C. C. Chamis, “Progressive Damage and Fracture of
Unstiffened and Stiffened Composite Pressure Vessels,” Journal of Reinforced Plastics and Composites, Vol.16, pp. 17111724, 1997.
[28] J. Triplett, J. Patterson, J. R. Esslinger and J. Zalameda, “Impact Damage
Evaluation of Stiffened Graphite Epoxy Cylinders,” American Institute of Aeronautics and Astronautics, AIAA981787, pp.18091813, 1998.
[29] R. Veys, A. Cederberg and J. Schimenti, “Fatigue Analysis Techniques for
Composite Tankage with Plastically Operating Aluminum Liners,” AIAA, SAE, ASME, and ASEE, Joint Propulsion Conference, 27th, Sacramento, CA; United States; Vol.8, pp.2426, 1991.
[30] B. Su and G. S. Bhuyan, “Fracture Analyses on the Allmetal Cylinders and the
Metallined Hoopwrapped Cylinders with Axial Cracks,” The International Journal of Pressure Vessels and Piping, Vol.76, pp.677684, 1999.
[31] C. Kaynak and O. Mat, “Uniaxial Fatigue Behavior of Filamentwound Glass
fiber/epoxy Composite Tubes,” Composites Science and Technology, Vol. 61, pp. 18331840, 2001.
[32] N. Tarakc, L. Gemi and A. Yapici, “Fatigue Failure Behavior of Glass/epoxy ±55
Filament Wound Pipes under Internal Pressure,” Composites Science and Technology, Vol.65, pp.703708, 2005.
[33] A. R. Shahani and M. M. Kheirikhah, “Stress Intensity Factor Calculation of Steel
lined Hoopwrapped Cylinders with Internal Semielliptical Circumferential Crack,” Engineering Fracture Mechanics, Vol.74, pp. 20042013, 2007.
[34] M. A. Guerrero, C. Betegon and J. Belzunce, “Fracture Analysis of a Pressure
Vessel Made of High Strength Steel (HSS),” Engineering Failure Analysis, Vol.15, pp.208219, 2008.
133
VITA
Jianbing Hu was born on August 24th, 1979 in Xiaogan, Hubei, People’s Republic
China. He joined Wuhan University of Technology, in Wuhan, China and obtained his
B.E. degree in Mechanical Engineering in 2000. He then joined Huazhong University of
Science & Technology, in Hubei, China in 2001 and obtained his M.S. degree in
Mechanical Engineering in 2004. Jianbing Hu later enrolled for his Ph.D. in Mechanical
Engineering at Missouri S&T since August 2004. He has held the position of Graduate
Teaching Assistant since August 2004 to May 2005 at Missouri S&T in the Department
of Mechanical and Aerospace Engineering and also held the position of Graduate
Research Assistant since August 2004 to December 2008. He obtained his Ph.D. degree
in Mechanical Engineering in Spring 2009 at Missouri S&T.